#------------------------------------------------------------------------------
#$Date: 2016-02-14 16:26:36 +0200 (Sun, 14 Feb 2016) $
#$Revision: 176435 $
#$URL: svn://www.crystallography.net/cod/cif/2/10/52/2105270.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2105270
loop_
_publ_author_name
'García-Tuñón, Esther'
'Dacuña, Bruno'
'Zaragoza, Guillermo'
'Franco, Jaime'
'Guitián, Francisco'
_publ_section_title
;
 Cl--OH ion-exchanging process in chlorapatite
 (Ca₅(PO₄)₃Clₓ(OH)~1{-~x}) -- a deep insight
;
_journal_coeditor_code           ZB5021
_journal_issue                   5
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              467
_journal_page_last               479
_journal_paper_doi               10.1107/S0108768112019520
_journal_volume                  68
_journal_year                    2012
_chemical_compound_source        'synthesis as described'
_chemical_formula_moiety         'Ca5 Cl1 O12 P3'
_chemical_formula_sum            'Ca5 Cl O12 P3'
_chemical_formula_weight         520.76
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_conform_dict_location     ftp://ftp.iucr.org/pub/cif_core.dic
_audit_conform_dict_name         cif_core.dic
_audit_conform_dict_version      2.3
_audit_creation_date             2010-10-04T11:32:09-00:00
_audit_creation_method           'WinGX routine CIF_UPDATE'
_cell_angle_alpha                90
_cell_angle_beta                 120.0030(10)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.6430(3)
_cell_length_b                   6.7641(2)
_cell_length_c                   19.2882(6)
_cell_measurement_reflns_used    1997
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      27.35
_cell_measurement_theta_min      3.87
_cell_measurement_wavelength     0.71073
_cell_volume                     1089.51(6)
_computing_cell_refinement       'APPEX2 (BRUKER AXS, 2005)'
_computing_data_collection       'APPEX2 (BRUKER AXS, 2005)'
_computing_data_reduction        'APPEX2 (BRUKER AXS, 2005)'
_computing_molecular_graphics    'Ortep-3 for Windows (Farrugia, 1997)'
_computing_publication_material  'WinGX publication routines (Farrugia, 1999)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SIR2004 (Giacovazzo et al, 2004)'
_diffrn_ambient_temperature      298(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'BRUKER APPEX-II CCD'
_diffrn_measurement_method       'omega and phi scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.7107
_diffrn_reflns_av_R_equivalents  0.0271
_diffrn_reflns_av_unetI/netI     0.0213
_diffrn_reflns_limit_h_max       10
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            11773
_diffrn_reflns_theta_full        26.37
_diffrn_reflns_theta_max         26.37
_diffrn_reflns_theta_min         2.44
_exptl_absorpt_coefficient_mu    3.212
_exptl_absorpt_correction_T_max  1
_exptl_absorpt_correction_T_min  0.6816
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'BRUKER SADABS'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    3.175
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             1032
_exptl_crystal_size_max          0.29
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.10
_refine_diff_density_max         0.442
_refine_diff_density_min         -0.522
_refine_diff_density_rms         0.119
_refine_ls_extinction_coef       0.0407(11)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.059
_refine_ls_matrix_type           full
_refine_ls_number_parameters     201
_refine_ls_number_reflns         2208
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.059
_refine_ls_R_factor_all          0.0369
_refine_ls_R_factor_gt           0.0232
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.015
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0344P)²+1.3169P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0666
_refine_ls_wR_factor_ref         0.0755
_reflns_number_gt                1255
_reflns_number_total             2208
_reflns_threshold_expression     >2σ(I)
_cod_data_source_file            zb5021.cif
_cod_data_source_block           E_mono
_cod_original_sg_symbol_H-M      'P 21/c'
_cod_original_formula_sum        'Ca5 Cl1 O12 P3'
_cod_database_code               2105270
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_group
Ca1 Ca 0.74421(6) 1.25000(13) 0.00219(3) 0.01100(16) Uani 1 1 d . .
Ca2 Ca 0.66670(12) 0.99695(10) 0.16667(5) 0.0118(2) Uani 1 1 d . .
Ca3 Ca 0.66656(11) 0.50371(9) 0.16662(5) 0.0101(2) Uani 1 1 d . .
Ca4 Ca 0.26013(6) 0.24994(13) 0.12786(3) 0.01097(16) Uani 1 1 d . .
Ca5 Ca 0.00431(6) 0.74991(12) 0.13005(3) 0.01085(16) Uani 1 1 d . .
O1 O 0.9133(3) 1.0672(4) 0.13323(15) 0.0158(6) Uani 1 1 d . .
O2 O 0.8728(2) 1.2499(4) 0.23264(11) 0.0146(4) Uani 1 1 d . .
O3 O 0.5924(2) 1.2495(5) 0.06367(11) 0.0139(4) Uani 1 1 d . .
O4 O 0.3531(3) 1.0670(4) 0.04315(15) 0.0194(6) Uani 1 1 d . .
O5 O 0.5349(2) 1.2493(5) 0.20390(11) 0.0137(4) Uani 1 1 d . .
O6 O 0.7330(3) 1.0672(4) 0.32328(16) 0.0154(6) Uani 1 1 d . .
O7 O 0.6565(2) 0.7494(4) 0.07413(11) 0.0135(4) Uani 1 1 d . .
O8 O 0.8520(2) 0.7499(4) 0.25415(11) 0.0135(4) Uani 1 1 d . .
O9 O 0.4920(2) 0.7508(4) 0.17181(12) 0.0136(4) Uani 1 1 d . .
O10 O 0.9134(3) 0.4326(4) 0.13347(16) 0.0217(6) Uani 1 1 d . .
O11 O 0.7333(3) 0.4326(4) 0.32332(18) 0.0230(7) Uani 1 1 d . .
O12 O 0.3535(3) 0.4328(4) 0.04349(16) 0.0187(6) Uani 1 1 d . .
P1 P 0.96750(8) 1.25012(16) 0.18748(4) 0.00720(18) Uani 1 1 d . .
P2 P 0.40738(8) 1.24998(16) 0.01626(4) 0.00720(18) Uani 1 1 d . .
P3 P 0.62525(8) 1.25028(15) 0.29632(4) 0.00716(18) Uani 1 1 d . .
Cl1A Cl 0.0011(4) 0.5562(4) -0.00127(18) 0.0264(10) Uani 0.501(4) 1 d P 1
Cl1B Cl -0.0010(4) 0.9443(4) 0.00127(18) 0.0260(10) Uani 0.499(4) 1 d P 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.1484 0.1585 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.006 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Ca1 O4 87.21(9) . 3_675
O3 Ca1 O12 87.41(9) . 3_675
O4 Ca1 O12 133.99(8) 3_675 3_675
O3 Ca1 O1 75.14(8) . .
O4 Ca1 O1 82.14(9) 3_675 .
O12 Ca1 O1 139.53(9) 3_675 .
O3 Ca1 O10 75.17(8) . 1_565
O4 Ca1 O10 139.34(9) 3_675 1_565
O12 Ca1 O10 82.30(10) 3_675 1_565
O1 Ca1 O10 58.18(6) . 1_565
O3 Ca1 Cl1A 142.47(9) . 3_675
O4 Ca1 Cl1A 128.36(8) 3_675 3_675
O12 Ca1 Cl1A 75.89(8) 3_675 3_675
O1 Ca1 Cl1A 96.07(8) . 3_675
O10 Ca1 Cl1A 69.51(8) 1_565 3_675
O3 Ca1 Cl1B 143.21(9) . 3_675
O4 Ca1 Cl1B 75.93(9) 3_675 3_675
O12 Ca1 Cl1B 127.65(7) 3_675 3_675
O1 Ca1 Cl1B 70.37(7) . 3_675
O10 Ca1 Cl1B 96.65(9) 1_565 3_675
Cl1A Ca1 Cl1B 55.65(5) 3_675 3_675
O3 Ca1 O9 104.88(6) . 3_675
O4 Ca1 O9 68.68(9) 3_675 3_675
O12 Ca1 O9 68.76(9) 3_675 3_675
O1 Ca1 O9 150.71(9) . 3_675
O10 Ca1 O9 150.96(9) 1_565 3_675
Cl1A Ca1 O9 100.01(7) 3_675 3_675
Cl1B Ca1 O9 99.10(8) 3_675 3_675
O3 Ca1 P1 70.21(5) . .
O4 Ca1 P1 110.40(7) 3_675 .
O12 Ca1 P1 110.48(7) 3_675 .
O1 Ca1 P1 29.25(6) . .
O10 Ca1 P1 29.16(6) 1_565 .
Cl1A Ca1 P1 84.35(6) 3_675 .
Cl1B Ca1 P1 85.20(7) 3_675 .
O9 Ca1 P1 175.09(4) 3_675 .
O3 Ca1 Cl1B 133.37(9) . 1_655
O4 Ca1 Cl1B 64.64(9) 3_675 1_655
O12 Ca1 Cl1B 138.99(7) 3_675 1_655
O1 Ca1 Cl1B 65.21(7) . 1_655
O10 Ca1 Cl1B 101.90(9) 1_565 1_655
Cl1A Ca1 Cl1B 67.99(9) 3_675 1_655
Cl1B Ca1 Cl1B 12.38(9) 3_675 1_655
O9 Ca1 Cl1B 98.57(7) 3_675 1_655
P1 Ca1 Cl1B 85.12(6) . 1_655
O3 Ca1 Cl1A 134.34(9) . 1_665
O4 Ca1 Cl1A 138.26(8) 3_675 1_665
O12 Ca1 Cl1A 64.84(8) 3_675 1_665
O1 Ca1 Cl1A 102.33(8) . 1_665
O10 Ca1 Cl1A 66.14(7) 1_565 1_665
Cl1A Ca1 Cl1A 11.54(10) 3_675 1_665
Cl1B Ca1 Cl1A 67.15(8) 3_675 1_665
O9 Ca1 Cl1A 98.02(7) 3_675 1_665
P1 Ca1 Cl1A 85.81(6) . 1_665
Cl1B Ca1 Cl1A 79.50(5) 1_655 1_665
O3 Ca1 P2 22.56(5) . .
O4 Ca1 P2 78.92(6) 3_675 .
O12 Ca1 P2 78.93(6) 3_675 .
O1 Ca1 P2 94.84(6) . .
O10 Ca1 P2 94.79(6) 1_565 .
Cl1A Ca1 P2 151.78(6) 3_675 .
Cl1B Ca1 P2 152.25(6) 3_675 .
O9 Ca1 P2 82.32(4) 3_675 .
P1 Ca1 P2 92.77(2) . .
Cl1B Ca1 P2 139.88(6) 1_655 .
Cl1A Ca1 P2 140.41(6) 1_665 .
O9 Ca2 O8 77.32(8) . .
O9 Ca2 O7 77.28(8) . .
O8 Ca2 O7 77.21(8) . .
O9 Ca2 O3 126.26(8) . .
O8 Ca2 O3 150.21(7) . .
O7 Ca2 O3 89.82(9) . .
O9 Ca2 O5 89.63(9) . .
O8 Ca2 O5 126.25(8) . .
O7 Ca2 O5 150.26(8) . .
O3 Ca2 O5 76.46(8) . .
O9 Ca2 O2 150.16(7) . .
O8 Ca2 O2 89.76(9) . .
O7 Ca2 O2 126.36(8) . .
O3 Ca2 O2 76.41(8) . .
O5 Ca2 O2 76.38(8) . .
O9 Ca2 O6 81.94(7) . .
O8 Ca2 O6 70.91(7) . .
O7 Ca2 O6 145.01(8) . .
O3 Ca2 O6 125.14(8) . .
O5 Ca2 O6 55.60(7) . .
O2 Ca2 O6 68.37(7) . .
O9 Ca2 O1 145.12(8) . .
O8 Ca2 O1 82.03(8) . .
O7 Ca2 O1 70.88(7) . .
O3 Ca2 O1 68.34(7) . .
O5 Ca2 O1 125.21(8) . .
O2 Ca2 O1 55.76(7) . .
O6 Ca2 O1 117.27(8) . .
O9 Ca2 O4 70.83(8) . .
O8 Ca2 O4 145.04(9) . .
O7 Ca2 O4 82.00(8) . .
O3 Ca2 O4 55.69(7) . .
O5 Ca2 O4 68.43(7) . .
O2 Ca2 O4 125.16(8) . .
O6 Ca2 O4 117.16(7) . .
O1 Ca2 O4 117.12(7) . .
O9 Ca2 P1 165.90(7) . .
O8 Ca2 P1 88.59(6) . .
O7 Ca2 P1 99.34(6) . .
O3 Ca2 P1 66.93(5) . .
O5 Ca2 P1 99.25(6) . .
O2 Ca2 P1 27.62(4) . .
O6 Ca2 P1 94.01(6) . .
O1 Ca2 P1 28.47(5) . .
O4 Ca2 P1 122.62(6) . .
O9 Ca2 P2 99.26(6) . .
O8 Ca2 P2 165.84(6) . .
O7 Ca2 P2 88.64(6) . .
O3 Ca2 P2 27.59(5) . .
O5 Ca2 P2 66.97(5) . .
O2 Ca2 P2 99.22(6) . .
O6 Ca2 P2 122.57(6) . .
O1 Ca2 P2 93.94(6) . .
O4 Ca2 P2 28.44(5) . .
P1 Ca2 P2 94.31(3) . .
O9 Ca2 P3 88.56(6) . .
O8 Ca2 P3 99.31(6) . .
O7 Ca2 P3 165.83(6) . .
O3 Ca2 P3 99.20(6) . .
O5 Ca2 P3 27.55(5) . .
O2 Ca2 P3 66.85(5) . .
O6 Ca2 P3 28.41(5) . .
O1 Ca2 P3 122.61(6) . .
O4 Ca2 P3 94.03(5) . .
P1 Ca2 P3 94.26(3) . .
P2 Ca2 P3 94.30(3) . .
O7 Ca3 O9 77.39(8) . .
O7 Ca3 O8 77.45(8) . .
O9 Ca3 O8 77.33(8) . .
O7 Ca3 O2 126.27(8) . 1_545
O9 Ca3 O2 150.19(7) . 1_545
O8 Ca3 O2 89.71(9) . 1_545
O7 Ca3 O3 89.80(9) . 1_545
O9 Ca3 O3 126.45(8) . 1_545
O8 Ca3 O3 150.19(7) . 1_545
O2 Ca3 O3 76.18(8) 1_545 1_545
O7 Ca3 O5 150.30(8) . 1_545
O9 Ca3 O5 89.98(9) . 1_545
O8 Ca3 O5 126.29(8) . 1_545
O2 Ca3 O5 76.12(8) 1_545 1_545
O3 Ca3 O5 76.15(8) 1_545 1_545
O7 Ca3 O12 82.10(8) . .
O9 Ca3 O12 70.99(8) . .
O8 Ca3 O12 145.30(9) . .
O2 Ca3 O12 124.95(8) 1_545 .
O3 Ca3 O12 55.72(7) 1_545 .
O5 Ca3 O12 68.34(7) 1_545 .
O7 Ca3 O10 70.88(8) . .
O9 Ca3 O10 145.15(8) . .
O8 Ca3 O10 82.00(8) . .
O2 Ca3 O10 55.64(7) 1_545 .
O3 Ca3 O10 68.33(8) 1_545 .
O5 Ca3 O10 124.84(8) 1_545 .
O12 Ca3 O10 117.19(8) . .
O7 Ca3 O11 145.30(9) . .
O9 Ca3 O11 82.10(8) . .
O8 Ca3 O11 70.89(8) . .
O2 Ca3 O11 68.25(7) 1_545 .
O3 Ca3 O11 124.85(9) 1_545 .
O5 Ca3 O11 55.64(7) 1_545 .
O12 Ca3 O11 117.10(7) . .
O10 Ca3 O11 117.04(8) . .
O7 Ca3 P3 166.04(6) . 1_545
O9 Ca3 P3 88.66(6) . 1_545
O8 Ca3 P3 99.23(6) . 1_545
O2 Ca3 P3 66.80(5) 1_545 1_545
O3 Ca3 P3 99.03(6) 1_545 1_545
O5 Ca3 P3 27.60(5) 1_545 1_545
O12 Ca3 P3 93.91(5) . 1_545
O10 Ca3 P3 122.44(6) . 1_545
O11 Ca3 P3 28.35(6) . 1_545
O7 Ca3 P2 88.56(6) . 1_545
O9 Ca3 P2 99.41(6) . 1_545
O8 Ca3 P2 166.00(6) . 1_545
O2 Ca3 P2 99.06(6) 1_545 1_545
O3 Ca3 P2 27.61(5) 1_545 1_545
O5 Ca3 P2 66.86(5) 1_545 1_545
O12 Ca3 P2 28.42(5) . 1_545
O10 Ca3 P2 93.93(6) . 1_545
O11 Ca3 P2 122.49(6) . 1_545
P3 Ca3 P2 94.26(3) 1_545 1_545
O7 Ca3 P1 99.23(6) . 1_545
O9 Ca3 P1 165.82(7) . 1_545
O8 Ca3 P1 88.50(6) . 1_545
O2 Ca3 P1 27.61(4) 1_545 1_545
O3 Ca3 P1 66.82(5) 1_545 1_545
O5 Ca3 P1 98.98(6) 1_545 1_545
O12 Ca3 P1 122.53(6) . 1_545
O10 Ca3 P1 28.36(5) . 1_545
O11 Ca3 P1 93.86(6) . 1_545
P3 Ca3 P1 94.20(3) 1_545 1_545
P2 Ca3 P1 94.23(3) 1_545 1_545
O5 Ca4 O6 87.32(10) 1_545 2_645
O5 Ca4 O11 87.18(11) 1_545 2_645
O6 Ca4 O11 133.99(8) 2_645 2_645
O5 Ca4 O12 75.22(9) 1_545 .
O6 Ca4 O12 82.15(8) 2_645 .
O11 Ca4 O12 139.46(8) 2_645 .
O5 Ca4 O4 75.22(9) 1_545 1_545
O6 Ca4 O4 139.43(8) 2_645 1_545
O11 Ca4 O4 82.21(8) 2_645 1_545
O12 Ca4 O4 58.24(6) . 1_545
O5 Ca4 Cl1B 142.40(9) 1_545 3_565
O6 Ca4 Cl1B 128.28(9) 2_645 3_565
O11 Ca4 Cl1B 76.16(9) 2_645 3_565
O12 Ca4 Cl1B 95.88(8) . 3_565
O4 Ca4 Cl1B 69.34(9) 1_545 3_565
O5 Ca4 Cl1A 143.40(9) 1_545 3_565
O6 Ca4 Cl1A 75.72(9) 2_645 3_565
O11 Ca4 Cl1A 127.78(9) 2_645 3_565
O12 Ca4 Cl1A 70.54(8) . 3_565
O4 Ca4 Cl1A 96.88(9) 1_545 3_565
Cl1B Ca4 Cl1A 55.64(5) 3_565 3_565
O5 Ca4 O8 104.85(6) 1_545 2_645
O6 Ca4 O8 68.77(8) 2_645 2_645
O11 Ca4 O8 68.71(8) 2_645 2_645
O12 Ca4 O8 150.81(9) . 2_645
O4 Ca4 O8 150.81(9) 1_545 2_645
Cl1B Ca4 O8 100.11(7) 3_565 2_645
Cl1A Ca4 O8 98.89(7) 3_565 2_645
O5 Ca4 P2 70.29(5) 1_545 1_545
O6 Ca4 P2 110.40(6) 2_645 1_545
O11 Ca4 P2 110.45(7) 2_645 1_545
O12 Ca4 P2 29.23(6) . 1_545
O4 Ca4 P2 29.24(6) 1_545 1_545
Cl1B Ca4 P2 84.17(5) 3_565 1_545
Cl1A Ca4 P2 85.40(5) 3_565 1_545
O8 Ca4 P2 175.14(4) 2_645 1_545
O5 Ca4 Cl1A 133.68(9) 1_545 .
O6 Ca4 Cl1A 65.01(9) 2_645 .
O11 Ca4 Cl1A 138.87(9) 2_645 .
O12 Ca4 Cl1A 65.20(8) . .
O4 Ca4 Cl1A 101.59(8) 1_545 .
Cl1B Ca4 Cl1A 67.49(9) 3_565 .
Cl1A Ca4 Cl1A 11.92(11) 3_565 .
O8 Ca4 Cl1A 98.81(7) 2_645 .
P2 Ca4 Cl1A 84.91(5) 1_545 .
O5 Ca4 Cl1B 134.06(10) 1_545 1_545
O6 Ca4 Cl1B 138.48(9) 2_645 1_545
O11 Ca4 Cl1B 64.50(9) 2_645 1_545
O12 Ca4 Cl1B 102.68(8) . 1_545
O4 Ca4 Cl1B 66.10(8) 1_545 1_545
Cl1B Ca4 Cl1B 12.09(9) 3_565 1_545
Cl1A Ca4 Cl1B 67.66(9) 3_565 1_545
O8 Ca4 Cl1B 97.72(7) 2_645 1_545
P2 Ca4 Cl1B 85.99(5) 1_545 1_545
Cl1A Ca4 Cl1B 79.53(5) . 1_545
O5 Ca4 P3 22.49(4) 1_545 1_545
O6 Ca4 P3 78.82(7) 2_645 1_545
O11 Ca4 P3 78.95(8) 2_645 1_545
O12 Ca4 P3 94.74(7) . 1_545
O4 Ca4 P3 94.89(7) 1_545 1_545
Cl1B Ca4 P3 152.02(6) 3_565 1_545
Cl1A Ca4 P3 152.01(7) 3_565 1_545
O8 Ca4 P3 82.36(4) 2_645 1_545
P2 Ca4 P3 92.78(2) 1_545 1_545
Cl1A Ca4 P3 140.09(6) . 1_545
Cl1B Ca4 P3 140.17(6) 1_545 1_545
O2 Ca5 O10 87.24(10) 2_645 1_455
O2 Ca5 O1 87.35(10) 2_645 1_455
O10 Ca5 O1 134.02(8) 1_455 1_455
O2 Ca5 O11 75.15(8) 2_645 2_655
O10 Ca5 O11 139.40(10) 1_455 2_655
O1 Ca5 O11 82.20(9) 1_455 2_655
O2 Ca5 O6 75.15(8) 2_645 2_645
O10 Ca5 O6 82.23(9) 1_455 2_645
O1 Ca5 O6 139.39(9) 1_455 2_645
O11 Ca5 O6 58.14(6) 2_655 2_645
O2 Ca5 Cl1B 142.74(10) 2_645 .
O10 Ca5 Cl1B 128.29(9) 1_455 .
O1 Ca5 Cl1B 75.51(8) 1_455 .
O11 Ca5 Cl1B 69.98(9) 2_655 .
O6 Ca5 Cl1B 96.65(8) 2_645 .
O2 Ca5 Cl1A 142.92(9) 2_645 .
O10 Ca5 Cl1A 76.35(8) 1_455 .
O1 Ca5 Cl1A 127.75(8) 1_455 .
O11 Ca5 Cl1A 96.02(8) 2_655 .
O6 Ca5 Cl1A 69.89(8) 2_645 .
Cl1B Ca5 Cl1A 55.63(5) . .
O2 Ca5 O7 104.89(6) 2_645 1_455
O10 Ca5 O7 68.68(9) 1_455 1_455
O1 Ca5 O7 68.81(8) 1_455 1_455
O11 Ca5 O7 150.91(9) 2_655 1_455
O6 Ca5 O7 150.80(9) 2_645 1_455
Cl1B Ca5 O7 99.37(8) . 1_455
Cl1A Ca5 O7 99.75(8) . 1_455
O2 Ca5 P3 70.22(5) 2_645 2_645
O10 Ca5 P3 110.46(8) 1_455 2_645
O1 Ca5 P3 110.37(7) 1_455 2_645
O11 Ca5 P3 29.16(7) 2_655 2_645
O6 Ca5 P3 29.22(6) 2_645 2_645
Cl1B Ca5 P3 84.94(7) . 2_645
Cl1A Ca5 P3 84.58(7) . 2_645
O7 Ca5 P3 175.11(4) 1_455 2_645
O2 Ca5 Cl1A 133.66(9) 2_645 3_565
O10 Ca5 Cl1A 64.40(8) 1_455 3_565
O1 Ca5 Cl1A 138.82(8) 1_455 3_565
O11 Ca5 Cl1A 102.43(8) 2_655 3_565
O6 Ca5 Cl1A 65.74(8) 2_645 3_565
Cl1B Ca5 Cl1A 68.25(8) . 3_565
Cl1A Ca5 Cl1A 12.63(8) . 3_565
O7 Ca5 Cl1A 98.03(7) 1_455 3_565
P3 Ca5 Cl1A 85.68(6) 2_645 3_565
O2 Ca5 Cl1B 134.03(10) 2_645 3_575
O10 Ca5 Cl1B 138.48(9) 1_455 3_575
O1 Ca5 Cl1B 65.06(8) 1_455 3_575
O11 Ca5 Cl1B 65.64(9) 2_655 3_575
O6 Ca5 Cl1B 101.79(8) 2_645 3_575
Cl1B Ca5 Cl1B 11.28(11) . 3_575
Cl1A Ca5 Cl1B 66.90(8) . 3_575
O7 Ca5 Cl1B 98.53(7) 1_455 3_575
P3 Ca5 Cl1B 85.25(6) 2_645 3_575
Cl1A Ca5 Cl1B 79.52(5) 3_565 3_575
O2 Ca5 P1 22.55(5) 2_645 2_645
O10 Ca5 P1 78.88(7) 1_455 2_645
O1 Ca5 P1 78.95(6) 1_455 2_645
O11 Ca5 P1 94.79(6) 2_655 2_645
O6 Ca5 P1 94.82(6) 2_645 2_645
Cl1B Ca5 P1 151.70(7) . 2_645
Cl1A Ca5 P1 152.34(6) . 2_645
O7 Ca5 P1 82.34(4) 1_455 2_645
P3 Ca5 P1 92.77(2) 2_645 2_645
Cl1A Ca5 P1 139.83(5) 3_565 2_645
Cl1B Ca5 P1 140.44(6) 3_575 2_645
P1 O1 Ca5 139.15(16) . 1_655
P1 O1 Ca1 96.69(13) . .
Ca5 O1 Ca1 118.99(10) 1_655 .
P1 O1 Ca2 91.06(10) . .
Ca5 O1 Ca2 102.95(9) 1_655 .
Ca1 O1 Ca2 96.62(8) . .
P1 O2 Ca5 122.68(11) . 2_655
P1 O2 Ca2 105.26(12) . .
Ca5 O2 Ca2 114.64(10) 2_655 .
P1 O2 Ca3 105.16(12) . 1_565
Ca5 O2 Ca3 114.60(10) 2_655 1_565
Ca2 O2 Ca3 89.01(7) . 1_565
P2 O3 Ca1 122.64(10) . .
P2 O3 Ca2 105.39(13) . .
Ca1 O3 Ca2 114.67(10) . .
P2 O3 Ca3 105.14(12) . 1_565
Ca1 O3 Ca3 114.48(10) . 1_565
Ca2 O3 Ca3 89.06(6) . 1_565
P2 O4 Ca1 139.35(13) . 3_675
P2 O4 Ca4 96.55(13) . 1_565
Ca1 O4 Ca4 118.94(9) 3_675 1_565
P2 O4 Ca2 91.05(12) . .
Ca1 O4 Ca2 102.99(11) 3_675 .
Ca4 O4 Ca2 96.51(8) 1_565 .
P3 O5 Ca4 122.79(10) . 1_565
P3 O5 Ca2 105.46(13) . .
Ca4 O5 Ca2 114.66(11) 1_565 .
P3 O5 Ca3 105.06(13) . 1_565
Ca4 O5 Ca3 114.36(10) 1_565 1_565
Ca2 O5 Ca3 88.99(6) . 1_565
P3 O6 Ca4 139.39(13) . 2_655
P3 O6 Ca5 96.54(12) . 2_655
Ca4 O6 Ca5 118.82(11) 2_655 2_655
P3 O6 Ca2 91.19(11) . .
Ca4 O6 Ca2 103.00(9) 2_655 .
Ca5 O6 Ca2 96.55(7) 2_655 .
P2 O7 Ca3 133.68(17) 3_675 .
P2 O7 Ca2 133.21(16) 3_675 .
Ca3 O7 Ca2 87.66(6) . .
P2 O7 Ca5 98.75(8) 3_675 1_655
Ca3 O7 Ca5 96.45(8) . 1_655
Ca2 O7 Ca5 96.31(8) . 1_655
P1 O8 Ca2 133.36(16) 2_745 .
P1 O8 Ca3 133.61(16) 2_745 .
Ca2 O8 Ca3 87.60(6) . .
P1 O8 Ca4 98.77(9) 2_745 2_655
Ca2 O8 Ca4 96.31(7) . 2_655
Ca3 O8 Ca4 96.33(7) . 2_655
P3 O9 Ca2 133.62(16) 2_645 .
P3 O9 Ca3 133.30(16) 2_645 .
Ca2 O9 Ca3 87.72(6) . .
P3 O9 Ca1 98.66(9) 2_645 3_675
Ca2 O9 Ca1 96.42(7) . 3_675
Ca3 O9 Ca1 96.26(7) . 3_675
P1 O10 Ca5 139.23(17) 1_545 1_655
P1 O10 Ca1 96.70(14) 1_545 1_545
Ca5 O10 Ca1 118.81(10) 1_655 1_545
P1 O10 Ca3 91.29(10) 1_545 .
Ca5 O10 Ca3 102.90(10) 1_655 .
Ca1 O10 Ca3 96.64(9) 1_545 .
P3 O11 Ca4 139.16(13) 1_545 2_655
P3 O11 Ca5 96.71(14) 1_545 2_645
Ca4 O11 Ca5 118.91(12) 2_655 2_645
P3 O11 Ca3 91.22(13) 1_545 .
Ca4 O11 Ca3 102.88(11) 2_655 .
Ca5 O11 Ca3 96.68(7) 2_645 .
P2 O12 Ca1 139.06(14) 1_545 3_675
P2 O12 Ca4 96.67(13) 1_545 .
Ca1 O12 Ca4 118.95(9) 3_675 .
P2 O12 Ca3 91.31(12) 1_545 .
Ca1 O12 Ca3 102.93(10) 3_675 .
Ca4 O12 Ca3 96.74(9) . .
O8 P1 O10 112.19(15) 2_755 1_565
O8 P1 O1 112.05(15) 2_755 .
O10 P1 O1 107.62(11) 1_565 .
O8 P1 O2 111.17(11) 2_755 .
O10 P1 O2 106.75(15) 1_565 .
O1 P1 O2 106.74(15) . .
O8 P1 Ca1 136.36(8) 2_755 .
O10 P1 Ca1 54.14(11) 1_565 .
O1 P1 Ca1 54.05(10) . .
O2 P1 Ca1 112.47(8) . .
O8 P1 Ca2 135.64(11) 2_755 .
O10 P1 Ca2 111.45(11) 1_565 .
O1 P1 Ca2 60.46(9) . .
O2 P1 Ca2 47.12(10) . .
Ca1 P1 Ca2 78.11(3) . .
O8 P1 Ca3 135.73(11) 2_755 1_565
O10 P1 Ca3 60.35(10) 1_565 1_565
O1 P1 Ca3 111.50(10) . 1_565
O2 P1 Ca3 47.23(10) . 1_565
Ca1 P1 Ca3 78.12(3) . 1_565
Ca2 P1 Ca3 64.380(18) . 1_565
O8 P1 Ca5 76.41(7) 2_755 2_655
O10 P1 Ca5 122.02(11) 1_565 2_655
O1 P1 Ca5 122.07(10) . 2_655
Ca1 P1 Ca5 147.23(2) . 2_655
Ca2 P1 Ca5 74.25(2) . 2_655
Ca3 P1 Ca5 74.30(2) 1_565 2_655
O8 P1 Ca4 55.96(7) 2_755 1_665
O10 P1 Ca4 80.50(10) 1_565 1_665
O1 P1 Ca4 80.38(9) . 1_665
O2 P1 Ca4 167.13(8) . 1_665
Ca1 P1 Ca4 80.404(19) . 1_665
Ca2 P1 Ca4 140.80(3) . 1_665
Ca3 P1 Ca4 140.81(3) 1_565 1_665
Ca5 P1 Ca4 132.36(2) 2_655 1_665
O4 P2 O7 112.12(15) . 3_675
O4 P2 O12 107.72(11) . 1_565
O7 P2 O12 112.07(15) 3_675 1_565
O4 P2 O3 106.67(16) . .
O7 P2 O3 111.22(11) 3_675 .
O12 P2 O3 106.72(16) 1_565 .
O4 P2 Ca4 54.21(9) . 1_565
O7 P2 Ca4 136.36(8) 3_675 1_565
O12 P2 Ca4 54.09(9) 1_565 1_565
O3 P2 Ca4 112.42(7) . 1_565
O4 P2 Ca2 60.51(12) . .
O7 P2 Ca2 135.82(11) 3_675 .
O12 P2 Ca2 111.36(11) 1_565 .
O3 P2 Ca2 47.02(10) . .
Ca4 P2 Ca2 78.12(2) 1_565 .
O4 P2 Ca3 111.64(10) . 1_565
O7 P2 Ca3 135.53(11) 3_675 1_565
O12 P2 Ca3 60.27(11) 1_565 1_565
O3 P2 Ca3 47.24(10) . 1_565
Ca4 P2 Ca3 78.13(2) 1_565 1_565
Ca2 P2 Ca3 64.386(18) . 1_565
O4 P2 Ca1 122.01(12) . .
O7 P2 Ca1 76.41(8) 3_675 .
O12 P2 Ca1 121.98(11) 1_565 .
Ca4 P2 Ca1 147.23(3) 1_565 .
Ca2 P2 Ca1 74.25(2) . .
Ca3 P2 Ca1 74.27(2) 1_565 .
O4 P2 Ca5 80.40(12) . 3_575
O7 P2 Ca5 55.93(7) 3_675 3_575
O12 P2 Ca5 80.55(11) 1_565 3_575
O3 P2 Ca5 167.14(7) . 3_575
Ca4 P2 Ca5 80.436(19) 1_565 3_575
Ca2 P2 Ca5 140.87(3) . 3_575
Ca3 P2 Ca5 140.78(3) 1_565 3_575
Ca1 P2 Ca5 132.34(2) . 3_575
O11 P3 O6 107.80(12) 1_565 .
O11 P3 O9 112.06(14) 1_565 2_655
O6 P3 O9 112.14(14) . 2_655
O11 P3 O5 106.98(16) 1_565 .
O6 P3 O5 106.50(15) . .
O9 P3 O5 111.07(11) 2_655 .
O11 P3 Ca5 54.14(11) 1_565 2_655
O6 P3 Ca5 54.24(10) . 2_655
O9 P3 Ca5 136.43(8) 2_655 2_655
O5 P3 Ca5 112.51(7) . 2_655
O11 P3 Ca3 60.44(11) 1_565 1_565
O6 P3 Ca3 111.61(8) . 1_565
O9 P3 Ca3 135.51(11) 2_655 1_565
O5 P3 Ca3 47.34(10) . 1_565
Ca5 P3 Ca3 78.19(3) 2_655 1_565
O11 P3 Ca2 111.48(9) 1_565 .
O6 P3 Ca2 60.40(10) . .
O9 P3 Ca2 135.71(11) 2_655 .
O5 P3 Ca2 46.99(10) . .
Ca5 P3 Ca2 78.12(3) 2_655 .
Ca3 P3 Ca2 64.379(17) 1_565 .
O11 P3 Ca4 122.09(13) 1_565 1_565
O6 P3 Ca4 121.86(12) . 1_565
O9 P3 Ca4 76.34(8) 2_655 1_565
Ca5 P3 Ca4 147.23(2) 2_655 1_565
Ca3 P3 Ca4 74.24(2) 1_565 1_565
Ca2 P3 Ca4 74.22(3) . 1_565
O11 P3 Ca1 80.49(11) 1_565 4_586
O6 P3 Ca1 80.46(10) . 4_586
O9 P3 Ca1 55.98(8) 2_655 4_586
O5 P3 Ca1 167.04(8) . 4_586
Ca5 P3 Ca1 80.449(19) 2_655 4_586
Ca3 P3 Ca1 140.88(4) 1_565 4_586
Ca2 P3 Ca1 140.83(3) . 4_586
Ca4 P3 Ca1 132.32(2) 1_565 4_586
Cl1A Cl1A Ca1 121.4(5) 3_565 3_675
Cl1A Cl1A Ca4 118.7(5) 3_565 3_565
Ca1 Cl1A Ca4 100.66(7) 3_675 3_565
Cl1A Cl1A Ca5 113.0(4) 3_565 .
Ca1 Cl1A Ca5 99.90(10) 3_675 .
Ca4 Cl1A Ca5 99.51(9) 3_565 .
Cl1A Cl1A Ca5 54.4(4) 3_565 3_565
Ca1 Cl1A Ca5 88.40(7) 3_675 3_565
Ca4 Cl1A Ca5 88.17(8) 3_565 3_565
Ca5 Cl1A Ca5 167.37(8) . 3_565
Cl1A Cl1A Ca4 49.4(4) 3_565 .
Ca1 Cl1A Ca4 87.86(8) 3_675 .
Ca4 Cl1A Ca4 168.08(11) 3_565 .
Ca5 Cl1A Ca4 87.07(8) . .
Ca5 Cl1A Ca4 83.72(6) 3_565 .
Cl1A Cl1A Ca1 47.0(4) 3_565 1_445
Ca1 Cl1A Ca1 168.46(10) 3_675 1_445
Ca4 Cl1A Ca1 87.35(8) 3_565 1_445
Ca5 Cl1A Ca1 86.80(6) . 1_445
Ca5 Cl1A Ca1 83.54(7) 3_565 1_445
Ca4 Cl1A Ca1 83.08(5) . 1_445
Cl1B Cl1B Ca5 122.6(4) 3_575 .
Cl1B Cl1B Ca4 116.6(5) 3_575 3_565
Ca5 Cl1B Ca4 100.40(8) . 3_565
Cl1B Cl1B Ca1 114.2(4) 3_575 3_675
Ca5 Cl1B Ca1 100.10(8) . 3_675
Ca4 Cl1B Ca1 99.32(9) 3_565 3_675
Cl1B Cl1B Ca1 53.4(4) 3_575 1_455
Ca5 Cl1B Ca1 88.40(7) . 1_455
Ca4 Cl1B Ca1 87.85(8) 3_565 1_455
Ca1 Cl1B Ca1 167.62(9) 3_675 1_455
Cl1B Cl1B Ca4 51.3(5) 3_575 1_565
Ca5 Cl1B Ca4 88.19(8) . 1_565
Ca4 Cl1B Ca4 167.91(9) 3_565 1_565
Ca1 Cl1B Ca4 87.39(9) 3_675 1_565
Ca1 Cl1B Ca4 83.88(7) 1_455 1_565
Cl1B Cl1B Ca5 46.2(4) 3_575 3_575
Ca5 Cl1B Ca5 168.72(11) . 3_575
Ca4 Cl1B Ca5 87.09(8) 3_565 3_575
Ca1 Cl1B Ca5 86.85(6) 3_675 3_575
Ca1 Cl1B Ca5 83.43(6) 1_455 3_575
Ca4 Cl1B Ca5 83.23(6) 1_565 3_575
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ca1 O3 2.2992(18) .
Ca1 O4 2.328(3) 3_675
Ca1 O12 2.332(3) 3_675
Ca1 O1 2.540(3) .
Ca1 O10 2.543(3) 1_565
Ca1 Cl1A 2.792(3) 3_675
Ca1 Cl1B 2.834(3) 3_675
Ca1 O9 2.967(2) 3_675
Ca1 P1 3.1166(8) .
Ca1 Cl1B 3.218(3) 1_655
Ca1 Cl1A 3.255(3) 1_665
Ca1 P2 3.3920(8) .
Ca2 O9 2.406(2) .
Ca2 O8 2.412(3) .
Ca2 O7 2.413(3) .
Ca2 O3 2.440(3) .
Ca2 O5 2.441(3) .
Ca2 O2 2.443(3) .
Ca2 O6 2.798(3) .
Ca2 O1 2.799(2) .
Ca2 O4 2.800(3) .
Ca2 P1 3.2160(12) .
Ca2 P2 3.2161(12) .
Ca2 P3 3.2171(10) .
Ca3 O7 2.404(2) .
Ca3 O9 2.409(2) .
Ca3 O8 2.408(3) .
Ca3 O2 2.448(3) 1_545
Ca3 O3 2.448(3) 1_545
Ca3 O5 2.450(3) 1_545
Ca3 O12 2.795(3) .
Ca3 O10 2.798(3) .
Ca3 O11 2.799(3) .
Ca3 P3 3.2174(10) 1_545
Ca3 P2 3.2178(12) 1_545
Ca3 P1 3.2184(11) 1_545
Ca4 O5 2.299(2) 1_545
Ca4 O6 2.331(3) 2_645
Ca4 O11 2.332(3) 2_645
Ca4 O12 2.541(2) .
Ca4 O4 2.544(2) 1_545
Ca4 Cl1B 2.819(3) 3_565
Ca4 Cl1A 2.806(3) 3_565
Ca4 O8 2.9679(19) 2_645
Ca4 P2 3.1154(8) 1_545
Ca4 Cl1A 3.242(3) .
Ca4 Cl1B 3.229(3) 1_545
Ca4 P3 3.3931(8) 1_545
Ca5 O2 2.2978(19) 2_645
Ca5 O10 2.332(3) 1_455
Ca5 O1 2.331(3) 1_455
Ca5 O11 2.542(3) 2_655
Ca5 O6 2.544(3) 2_645
Ca5 Cl1B 2.788(2) .
Ca5 Cl1A 2.838(3) .
Ca5 O7 2.965(2) 1_455
Ca5 P3 3.1151(8) 2_645
Ca5 Cl1A 3.214(3) 3_565
Ca5 Cl1B 3.258(2) 3_575
Ca5 P1 3.3918(8) 2_645
O1 P1 1.533(3) .
O1 Ca5 2.331(3) 1_655
O2 P1 1.5455(18) .
O2 Ca5 2.2978(19) 2_655
O2 Ca3 2.448(3) 1_565
O3 P2 1.5451(19) .
O3 Ca3 2.448(3) 1_565
O4 P2 1.532(3) .
O4 Ca1 2.328(3) 3_675
O4 Ca4 2.544(2) 1_565
O5 P3 1.5439(19) .
O5 Ca4 2.299(2) 1_565
O5 Ca3 2.450(3) 1_565
O6 P3 1.531(3) .
O6 Ca4 2.331(3) 2_655
O6 Ca5 2.544(3) 2_655
O7 P2 1.5314(18) 3_675
O7 Ca5 2.965(2) 1_655
O8 P1 1.5290(19) 2_745
O8 Ca4 2.9679(19) 2_655
O9 P3 1.5333(17) 2_645
O9 Ca1 2.967(2) 3_675
O10 P1 1.529(3) 1_545
O10 Ca5 2.332(3) 1_655
O10 Ca1 2.543(3) 1_545
O11 P3 1.528(3) 1_545
O11 Ca4 2.332(3) 2_655
O11 Ca5 2.542(3) 2_645
O12 P2 1.532(3) 1_545
O12 Ca1 2.332(3) 3_675
P1 O8 1.5290(19) 2_755
P1 O10 1.529(3) 1_565
P1 Ca3 3.2184(11) 1_565
P1 Ca5 3.3918(8) 2_655
P2 O7 1.5314(18) 3_675
P2 O12 1.532(3) 1_565
P2 Ca4 3.1154(8) 1_565
P2 Ca3 3.2178(12) 1_565
P3 O11 1.528(3) 1_565
P3 O9 1.5333(17) 2_655
P3 Ca5 3.1151(8) 2_655
P3 Ca3 3.2174(10) 1_565
P3 Ca4 3.3931(8) 1_565
Cl1A Cl1A 0.763(5) 3_565
Cl1A Ca1 2.792(3) 3_675
Cl1A Ca4 2.806(3) 3_565
Cl1A Ca5 3.214(3) 3_565
Cl1A Ca1 3.255(3) 1_445
Cl1B Cl1B 0.756(5) 3_575
Cl1B Ca4 2.819(3) 3_565
Cl1B Ca1 2.834(3) 3_675
Cl1B Ca1 3.218(3) 1_455
Cl1B Ca4 3.229(3) 1_565
Cl1B Ca5 3.258(2) 3_575
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O3 Ca1 O1 P1 -75.93(11) . .
O4 Ca1 O1 P1 -165.12(12) 3_675 .
O12 Ca1 O1 P1 -8.44(19) 3_675 .
O10 Ca1 O1 P1 5.61(8) 1_565 .
Cl1A Ca1 O1 P1 66.90(11) 3_675 .
Cl1B Ca1 O1 P1 117.08(12) 3_675 .
O9 Ca1 O1 P1 -169.95(8) 3_675 .
Cl1B Ca1 O1 P1 129.24(13) 1_655 .
Cl1A Ca1 O1 P1 57.08(11) 1_665 .
P2 Ca1 O1 P1 -87.03(10) . .
O3 Ca1 O1 Ca5 124.72(14) . 1_655
O4 Ca1 O1 Ca5 35.54(12) 3_675 1_655
O12 Ca1 O1 Ca5 -167.78(11) 3_675 1_655
O10 Ca1 O1 Ca5 -153.74(16) 1_565 1_655
Cl1A Ca1 O1 Ca5 -92.44(12) 3_675 1_655
Cl1B Ca1 O1 Ca5 -42.27(11) 3_675 1_655
O9 Ca1 O1 Ca5 30.7(2) 3_675 1_655
P1 Ca1 O1 Ca5 -159.35(19) . 1_655
Cl1B Ca1 O1 Ca5 -30.10(10) 1_655 1_655
Cl1A Ca1 O1 Ca5 -102.26(12) 1_665 1_655
P2 Ca1 O1 Ca5 113.62(10) . 1_655
O3 Ca1 O1 Ca2 15.93(9) . .
O4 Ca1 O1 Ca2 -73.26(8) 3_675 .
O12 Ca1 O1 Ca2 83.42(14) 3_675 .
O10 Ca1 O1 Ca2 97.47(10) 1_565 .
Cl1A Ca1 O1 Ca2 158.76(8) 3_675 .
Cl1B Ca1 O1 Ca2 -151.06(10) 3_675 .
O9 Ca1 O1 Ca2 -78.09(13) 3_675 .
P1 Ca1 O1 Ca2 91.86(11) . .
Cl1B Ca1 O1 Ca2 -138.90(10) 1_655 .
Cl1A Ca1 O1 Ca2 148.94(7) 1_665 .
P2 Ca1 O1 Ca2 4.83(7) . .
O9 Ca2 O1 P1 -155.84(12) . .
O8 Ca2 O1 P1 -101.87(12) . .
O7 Ca2 O1 P1 178.97(13) . .
O3 Ca2 O1 P1 81.26(12) . .
O5 Ca2 O1 P1 27.32(15) . .
O2 Ca2 O1 P1 -6.70(10) . .
O6 Ca2 O1 P1 -38.21(14) . .
O4 Ca2 O1 P1 109.03(12) . .
P2 Ca2 O1 P1 91.78(11) . .
P3 Ca2 O1 P1 -5.88(14) . .
O9 Ca2 O1 Ca5 -14.53(19) . 1_655
O8 Ca2 O1 Ca5 39.44(10) . 1_655
O7 Ca2 O1 Ca5 -39.72(9) . 1_655
O3 Ca2 O1 Ca5 -137.43(11) . 1_655
O5 Ca2 O1 Ca5 168.63(8) . 1_655
O2 Ca2 O1 Ca5 134.61(13) . 1_655
O6 Ca2 O1 Ca5 103.10(9) . 1_655
O4 Ca2 O1 Ca5 -109.66(10) . 1_655
P1 Ca2 O1 Ca5 141.31(17) . 1_655
P2 Ca2 O1 Ca5 -126.92(8) . 1_655
P3 Ca2 O1 Ca5 135.43(7) . 1_655
O9 Ca2 O1 Ca1 107.30(14) . .
O8 Ca2 O1 Ca1 161.26(9) . .
O7 Ca2 O1 Ca1 82.10(9) . .
O3 Ca2 O1 Ca1 -15.60(8) . .
O5 Ca2 O1 Ca1 -69.54(11) . .
O2 Ca2 O1 Ca1 -103.56(11) . .
O6 Ca2 O1 Ca1 -135.08(8) . .
O4 Ca2 O1 Ca1 12.17(11) . .
P1 Ca2 O1 Ca1 -96.86(13) . .
P2 Ca2 O1 Ca1 -5.09(7) . .
P3 Ca2 O1 Ca1 -102.75(7) . .
O9 Ca2 O2 P1 150.77(14) . .
O8 Ca2 O2 P1 87.40(13) . .
O7 Ca2 O2 P1 13.54(18) . .
O3 Ca2 O2 P1 -65.96(12) . .
O5 Ca2 O2 P1 -145.05(14) . .
O6 Ca2 O2 P1 156.90(15) . .
O1 Ca2 O2 P1 6.89(10) . .
O4 Ca2 O2 P1 -94.35(13) . .
P2 Ca2 O2 P1 -81.61(12) . .
P3 Ca2 O2 P1 -172.36(14) . .
O9 Ca2 O2 Ca5 13.0(2) . 2_655
O8 Ca2 O2 Ca5 -50.41(10) . 2_655
O7 Ca2 O2 Ca5 -124.27(10) . 2_655
O3 Ca2 O2 Ca5 156.23(11) . 2_655
O5 Ca2 O2 Ca5 77.14(10) . 2_655
O6 Ca2 O2 Ca5 19.09(9) . 2_655
O1 Ca2 O2 Ca5 -130.92(14) . 2_655
O4 Ca2 O2 Ca5 127.84(10) . 2_655
P1 Ca2 O2 Ca5 -137.8(2) . 2_655
P2 Ca2 O2 Ca5 140.58(9) . 2_655
P3 Ca2 O2 Ca5 49.83(8) . 2_655
O9 Ca2 O2 Ca3 -103.78(17) . 1_565
O8 Ca2 O2 Ca3 -167.15(7) . 1_565
O7 Ca2 O2 Ca3 118.99(9) . 1_565
O3 Ca2 O2 Ca3 39.48(6) . 1_565
O5 Ca2 O2 Ca3 -39.61(6) . 1_565
O6 Ca2 O2 Ca3 -97.65(8) . 1_565
O1 Ca2 O2 Ca3 112.34(9) . 1_565
O4 Ca2 O2 Ca3 11.09(9) . 1_565
P1 Ca2 O2 Ca3 105.45(13) . 1_565
P2 Ca2 O2 Ca3 23.84(5) . 1_565
P3 Ca2 O2 Ca3 -66.92(5) . 1_565
O4 Ca1 O3 P2 -67.4(2) 3_675 .
O12 Ca1 O3 P2 66.9(2) 3_675 .
O1 Ca1 O3 P2 -150.0(2) . .
O10 Ca1 O3 P2 149.6(2) 1_565 .
Cl1A Ca1 O3 P2 129.55(17) 3_675 .
Cl1B Ca1 O3 P2 -129.26(18) 3_675 .
O9 Ca1 O3 P2 -0.3(2) 3_675 .
P1 Ca1 O3 P2 179.8(2) . .
Cl1B Ca1 O3 P2 -117.90(18) 1_655 .
Cl1A Ca1 O3 P2 117.16(18) 1_665 .
O4 Ca1 O3 Ca2 62.47(12) 3_675 .
O12 Ca1 O3 Ca2 -163.24(12) 3_675 .
O1 Ca1 O3 Ca2 -20.13(10) . .
O10 Ca1 O3 Ca2 -80.52(10) 1_565 .
Cl1A Ca1 O3 Ca2 -100.59(17) 3_675 .
Cl1B Ca1 O3 Ca2 0.6(2) 3_675 .
O9 Ca1 O3 Ca2 129.55(10) 3_675 .
P1 Ca1 O3 Ca2 -50.38(8) . .
Cl1B Ca1 O3 Ca2 11.96(17) 1_655 .
Cl1A Ca1 O3 Ca2 -112.98(14) 1_665 .
P2 Ca1 O3 Ca2 129.9(3) . .
O4 Ca1 O3 Ca3 163.39(12) 3_675 1_565
O12 Ca1 O3 Ca3 -62.33(12) 3_675 1_565
O1 Ca1 O3 Ca3 80.78(10) . 1_565
O10 Ca1 O3 Ca3 20.39(10) 1_565 1_565
Cl1A Ca1 O3 Ca3 0.3(2) 3_675 1_565
Cl1B Ca1 O3 Ca3 101.52(18) 3_675 1_565
O9 Ca1 O3 Ca3 -129.54(10) 3_675 1_565
P1 Ca1 O3 Ca3 50.54(8) . 1_565
Cl1B Ca1 O3 Ca3 112.87(15) 1_655 1_565
Cl1A Ca1 O3 Ca3 -12.06(17) 1_665 1_565
P2 Ca1 O3 Ca3 -129.2(3) . 1_565
O9 Ca2 O3 P2 13.40(17) . .
O8 Ca2 O3 P2 150.60(14) . .
O7 Ca2 O3 P2 87.42(13) . .
O5 Ca2 O3 P2 -65.94(12) . .
O2 Ca2 O3 P2 -144.93(13) . .
O6 Ca2 O3 P2 -94.27(14) . .
O1 Ca2 O3 P2 156.86(15) . .
O4 Ca2 O3 P2 7.00(10) . .
P1 Ca2 O3 P2 -172.33(14) . .
P3 Ca2 O3 P2 -81.60(12) . .
O9 Ca2 O3 Ca1 -124.50(10) . .
O8 Ca2 O3 Ca1 12.7(2) . .
O7 Ca2 O3 Ca1 -50.48(11) . .
O5 Ca2 O3 Ca1 156.16(12) . .
O2 Ca2 O3 Ca1 77.17(10) . .
O6 Ca2 O3 Ca1 127.82(11) . .
O1 Ca2 O3 Ca1 18.96(9) . .
O4 Ca2 O3 Ca1 -130.91(14) . .
P1 Ca2 O3 Ca1 49.76(8) . .
P2 Ca2 O3 Ca1 -137.9(2) . .
P3 Ca2 O3 Ca1 140.49(9) . .
O9 Ca2 O3 Ca3 118.86(9) . 1_565
O8 Ca2 O3 Ca3 -103.95(17) . 1_565
O7 Ca2 O3 Ca3 -167.13(7) . 1_565
O5 Ca2 O3 Ca3 39.51(7) . 1_565
O2 Ca2 O3 Ca3 -39.48(6) . 1_565
O6 Ca2 O3 Ca3 11.18(10) . 1_565
O1 Ca2 O3 Ca3 -97.69(8) . 1_565
O4 Ca2 O3 Ca3 112.45(9) . 1_565
P1 Ca2 O3 Ca3 -66.88(5) . 1_565
P2 Ca2 O3 Ca3 105.45(13) . 1_565
P3 Ca2 O3 Ca3 23.85(5) . 1_565
O9 Ca2 O4 P2 178.66(12) . .
O8 Ca2 O4 P2 -155.85(11) . .
O7 Ca2 O4 P2 -102.08(11) . .
O3 Ca2 O4 P2 -6.80(9) . .
O5 Ca2 O4 P2 81.19(12) . .
O2 Ca2 O4 P2 27.22(13) . .
O6 Ca2 O4 P2 108.86(10) . .
O1 Ca2 O4 P2 -38.42(14) . .
P1 Ca2 O4 P2 -6.07(13) . .
P3 Ca2 O4 P2 91.59(10) . .
O9 Ca2 O4 Ca1 -39.80(8) . 3_675
O8 Ca2 O4 Ca1 -14.31(15) . 3_675
O7 Ca2 O4 Ca1 39.45(8) . 3_675
O3 Ca2 O4 Ca1 134.73(11) . 3_675
O5 Ca2 O4 Ca1 -137.28(10) . 3_675
O2 Ca2 O4 Ca1 168.75(7) . 3_675
O6 Ca2 O4 Ca1 -109.61(9) . 3_675
O1 Ca2 O4 Ca1 103.11(9) . 3_675
P1 Ca2 O4 Ca1 135.46(6) . 3_675
P2 Ca2 O4 Ca1 141.54(14) . 3_675
P3 Ca2 O4 Ca1 -126.87(6) . 3_675
O9 Ca2 O4 Ca4 81.95(8) . 1_565
O8 Ca2 O4 Ca4 107.43(13) . 1_565
O7 Ca2 O4 Ca4 161.20(9) . 1_565
O3 Ca2 O4 Ca4 -103.52(11) . 1_565
O5 Ca2 O4 Ca4 -15.53(8) . 1_565
O2 Ca2 O4 Ca4 -69.50(10) . 1_565
O6 Ca2 O4 Ca4 12.14(11) . 1_565
O1 Ca2 O4 Ca4 -135.14(8) . 1_565
P1 Ca2 O4 Ca4 -102.79(6) . 1_565
P2 Ca2 O4 Ca4 -96.72(13) . 1_565
P3 Ca2 O4 Ca4 -5.13(7) . 1_565
O9 Ca2 O5 P3 87.60(13) . .
O8 Ca2 O5 P3 13.67(18) . .
O7 Ca2 O5 P3 150.54(14) . .
O3 Ca2 O5 P3 -144.81(14) . .
O2 Ca2 O5 P3 -65.79(12) . .
O6 Ca2 O5 P3 7.13(10) . .
O1 Ca2 O5 P3 -94.21(14) . .
O4 Ca2 O5 P3 157.07(15) . .
P1 Ca2 O5 P3 -81.40(12) . .
P2 Ca2 O5 P3 -172.17(14) . .
O9 Ca2 O5 Ca4 -50.58(11) . 1_565
O8 Ca2 O5 Ca4 -124.51(10) . 1_565
O7 Ca2 O5 Ca4 12.4(2) . 1_565
O3 Ca2 O5 Ca4 77.01(11) . 1_565
O2 Ca2 O5 Ca4 156.03(12) . 1_565
O6 Ca2 O5 Ca4 -131.05(14) . 1_565
O1 Ca2 O5 Ca4 127.62(11) . 1_565
O4 Ca2 O5 Ca4 18.90(9) . 1_565
P1 Ca2 O5 Ca4 140.42(9) . 1_565
P2 Ca2 O5 Ca4 49.65(8) . 1_565
P3 Ca2 O5 Ca4 -138.2(2) . 1_565
O9 Ca2 O5 Ca3 -167.05(8) . 1_565
O8 Ca2 O5 Ca3 119.02(10) . 1_565
O7 Ca2 O5 Ca3 -104.11(16) . 1_565
O3 Ca2 O5 Ca3 -39.47(7) . 1_565
O2 Ca2 O5 Ca3 39.56(7) . 1_565
O6 Ca2 O5 Ca3 112.47(10) . 1_565
O1 Ca2 O5 Ca3 11.14(10) . 1_565
O4 Ca2 O5 Ca3 -97.58(7) . 1_565
P1 Ca2 O5 Ca3 23.95(5) . 1_565
P2 Ca2 O5 Ca3 -66.83(5) . 1_565
P3 Ca2 O5 Ca3 105.35(13) . 1_565
O9 Ca2 O6 P3 -102.04(12) . .
O8 Ca2 O6 P3 178.65(13) . .
O7 Ca2 O6 P3 -155.89(12) . .
O3 Ca2 O6 P3 27.07(15) . .
O5 Ca2 O6 P3 -6.93(10) . .
O2 Ca2 O6 P3 81.04(12) . .
O1 Ca2 O6 P3 108.74(12) . .
O4 Ca2 O6 P3 -38.49(13) . .
P1 Ca2 O6 P3 91.54(10) . .
P2 Ca2 O6 P3 -6.16(13) . .
O9 Ca2 O6 Ca4 39.60(9) . 2_655
O8 Ca2 O6 Ca4 -39.71(9) . 2_655
O7 Ca2 O6 Ca4 -14.25(19) . 2_655
O3 Ca2 O6 Ca4 168.71(8) . 2_655
O5 Ca2 O6 Ca4 134.71(13) . 2_655
O2 Ca2 O6 Ca4 -137.32(11) . 2_655
O1 Ca2 O6 Ca4 -109.62(10) . 2_655
O4 Ca2 O6 Ca4 103.15(10) . 2_655
P1 Ca2 O6 Ca4 -126.82(8) . 2_655
P2 Ca2 O6 Ca4 135.48(7) . 2_655
P3 Ca2 O6 Ca4 141.64(16) . 2_655
O9 Ca2 O6 Ca5 161.24(9) . 2_655
O8 Ca2 O6 Ca5 81.93(9) . 2_655
O7 Ca2 O6 Ca5 107.39(13) . 2_655
O3 Ca2 O6 Ca5 -69.65(11) . 2_655
O5 Ca2 O6 Ca5 -103.65(11) . 2_655
O2 Ca2 O6 Ca5 -15.68(8) . 2_655
O1 Ca2 O6 Ca5 12.02(11) . 2_655
O4 Ca2 O6 Ca5 -135.21(8) . 2_655
P1 Ca2 O6 Ca5 -5.18(7) . 2_655
P2 Ca2 O6 Ca5 -102.89(8) . 2_655
P3 Ca2 O6 Ca5 -96.72(12) . 2_655
O9 Ca3 O7 P2 -115.56(17) . 3_675
O8 Ca3 O7 P2 164.84(18) . 3_675
O2 Ca3 O7 P2 84.61(18) 1_545 3_675
O3 Ca3 O7 P2 12.00(16) 1_545 3_675
O5 Ca3 O7 P2 -48.7(3) 1_545 3_675
O12 Ca3 O7 P2 -43.37(16) . 3_675
O10 Ca3 O7 P2 79.07(17) . 3_675
O11 Ca3 O7 P2 -170.78(14) . 3_675
P3 Ca3 O7 P2 -117.5(3) 1_545 3_675
P2 Ca3 O7 P2 -15.59(16) 1_545 3_675
P1 Ca3 O7 P2 78.47(16) 1_545 3_675
O9 Ca3 O7 Ca2 39.72(7) . .
O8 Ca3 O7 Ca2 -39.88(7) . .
O2 Ca3 O7 Ca2 -120.11(10) 1_545 .
O3 Ca3 O7 Ca2 167.28(8) 1_545 .
O5 Ca3 O7 Ca2 106.57(16) 1_545 .
O12 Ca3 O7 Ca2 111.91(7) . .
O10 Ca3 O7 Ca2 -125.65(9) . .
O11 Ca3 O7 Ca2 -15.50(16) . .
P3 Ca3 O7 Ca2 37.7(3) 1_545 .
P2 Ca3 O7 Ca2 139.69(6) 1_545 .
P1 Ca3 O7 Ca2 -126.25(6) 1_545 .
O9 Ca3 O7 Ca5 135.81(8) . 1_655
O8 Ca3 O7 Ca5 56.20(7) . 1_655
O2 Ca3 O7 Ca5 -24.02(12) 1_545 1_655
O3 Ca3 O7 Ca5 -96.63(8) 1_545 1_655
O5 Ca3 O7 Ca5 -157.34(14) 1_545 1_655
O12 Ca3 O7 Ca5 -152.01(8) . 1_655
O10 Ca3 O7 Ca5 -29.57(8) . 1_655
O11 Ca3 O7 Ca5 80.59(15) . 1_655
P3 Ca3 O7 Ca5 133.8(2) 1_545 1_655
P2 Ca3 O7 Ca5 -124.22(6) 1_545 1_655
P1 Ca3 O7 Ca5 -30.17(7) 1_545 1_655
O9 Ca2 O7 P2 115.68(17) . 3_675
O8 Ca2 O7 P2 -164.66(17) . 3_675
O3 Ca2 O7 P2 -11.70(16) . 3_675
O5 Ca2 O7 P2 49.8(3) . 3_675
O2 Ca2 O7 P2 -84.59(18) . 3_675
O6 Ca2 O7 P2 170.72(13) . 3_675
O1 Ca2 O7 P2 -78.77(17) . 3_675
O4 Ca2 O7 P2 43.63(16) . 3_675
P1 Ca2 O7 P2 -78.27(16) . 3_675
P2 Ca2 O7 P2 15.87(16) . 3_675
P3 Ca2 O7 P2 118.1(3) . 3_675
O9 Ca2 O7 Ca3 -39.81(7) . .
O8 Ca2 O7 Ca3 39.86(7) . .
O3 Ca2 O7 Ca3 -167.18(8) . .
O5 Ca2 O7 Ca3 -105.71(16) . .
O2 Ca2 O7 Ca3 119.93(10) . .
O6 Ca2 O7 Ca3 15.24(15) . .
O1 Ca2 O7 Ca3 125.74(9) . .
O4 Ca2 O7 Ca3 -111.85(7) . .
P1 Ca2 O7 Ca3 126.24(6) . .
P2 Ca2 O7 Ca3 -139.61(6) . .
P3 Ca2 O7 Ca3 -37.3(3) . .
O9 Ca2 O7 Ca5 -136.04(8) . 1_655
O8 Ca2 O7 Ca5 -56.37(7) . 1_655
O3 Ca2 O7 Ca5 96.58(7) . 1_655
O5 Ca2 O7 Ca5 158.06(14) . 1_655
O2 Ca2 O7 Ca5 23.70(12) . 1_655
O6 Ca2 O7 Ca5 -80.99(15) . 1_655
O1 Ca2 O7 Ca5 29.51(7) . 1_655
O4 Ca2 O7 Ca5 151.92(8) . 1_655
P1 Ca2 O7 Ca5 30.01(7) . 1_655
P2 Ca2 O7 Ca5 124.16(6) . 1_655
P3 Ca2 O7 Ca5 -133.6(2) . 1_655
O9 Ca2 O8 P1 -164.67(17) . 2_745
O7 Ca2 O8 P1 115.72(16) . 2_745
O3 Ca2 O8 P1 49.5(3) . 2_745
O5 Ca2 O8 P1 -84.63(17) . 2_745
O2 Ca2 O8 P1 -11.79(16) . 2_745
O6 Ca2 O8 P1 -78.92(16) . 2_745
O1 Ca2 O8 P1 43.63(16) . 2_745
O4 Ca2 O8 P1 170.71(12) . 2_745
P1 Ca2 O8 P1 15.81(15) . 2_745
P2 Ca2 O8 P1 117.9(3) . 2_745
P3 Ca2 O8 P1 -78.27(15) . 2_745
O9 Ca2 O8 Ca3 39.83(6) . .
O7 Ca2 O8 Ca3 -39.78(6) . .
O3 Ca2 O8 Ca3 -106.00(17) . .
O5 Ca2 O8 Ca3 119.87(9) . .
O2 Ca2 O8 Ca3 -167.29(7) . .
O6 Ca2 O8 Ca3 125.58(8) . .
O1 Ca2 O8 Ca3 -111.87(7) . .
O4 Ca2 O8 Ca3 15.21(14) . .
P1 Ca2 O8 Ca3 -139.69(5) . .
P2 Ca2 O8 Ca3 -37.6(3) . .
P3 Ca2 O8 Ca3 126.22(5) . .
O9 Ca2 O8 Ca4 -56.27(7) . 2_655
O7 Ca2 O8 Ca4 -135.89(9) . 2_655
O3 Ca2 O8 Ca4 157.89(14) . 2_655
O5 Ca2 O8 Ca4 23.76(12) . 2_655
O2 Ca2 O8 Ca4 96.60(7) . 2_655
O6 Ca2 O8 Ca4 29.47(7) . 2_655
O1 Ca2 O8 Ca4 152.02(8) . 2_655
O4 Ca2 O8 Ca4 -80.89(13) . 2_655
P1 Ca2 O8 Ca4 124.20(6) . 2_655
P2 Ca2 O8 Ca4 -133.7(2) . 2_655
P3 Ca2 O8 Ca4 30.12(7) . 2_655
O7 Ca3 O8 P1 -115.48(16) . 2_745
O9 Ca3 O8 P1 164.84(17) . 2_745
O2 Ca3 O8 P1 11.91(16) 1_545 2_745
O3 Ca3 O8 P1 -48.8(3) 1_545 2_745
O5 Ca3 O8 P1 84.37(17) 1_545 2_745
O12 Ca3 O8 P1 -170.80(12) . 2_745
O10 Ca3 O8 P1 -43.40(16) . 2_745
O11 Ca3 O8 P1 78.92(17) . 2_745
P3 Ca3 O8 P1 78.33(16) 1_545 2_745
P2 Ca3 O8 P1 -117.2(3) 1_545 2_745
P1 Ca3 O8 P1 -15.68(15) 1_545 2_745
O7 Ca3 O8 Ca2 39.91(7) . .
O9 Ca3 O8 Ca2 -39.77(6) . .
O2 Ca3 O8 Ca2 167.30(7) 1_545 .
O3 Ca3 O8 Ca2 106.60(17) 1_545 .
O5 Ca3 O8 Ca2 -120.24(10) 1_545 .
O12 Ca3 O8 Ca2 -15.41(14) . .
O10 Ca3 O8 Ca2 112.00(7) . .
O11 Ca3 O8 Ca2 -125.69(8) . .
P3 Ca3 O8 Ca2 -126.27(5) 1_545 .
P2 Ca3 O8 Ca2 38.1(3) 1_545 .
P1 Ca3 O8 Ca2 139.71(5) 1_545 .
O7 Ca3 O8 Ca4 136.00(9) . 2_655
O9 Ca3 O8 Ca4 56.32(7) . 2_655
O2 Ca3 O8 Ca4 -96.61(7) 1_545 2_655
O3 Ca3 O8 Ca4 -157.32(15) 1_545 2_655
O5 Ca3 O8 Ca4 -24.15(12) 1_545 2_655
O12 Ca3 O8 Ca4 80.67(13) . 2_655
O10 Ca3 O8 Ca4 -151.92(9) . 2_655
O11 Ca3 O8 Ca4 -29.60(7) . 2_655
P3 Ca3 O8 Ca4 -30.19(7) 1_545 2_655
P2 Ca3 O8 Ca4 134.2(2) 1_545 2_655
P1 Ca3 O8 Ca4 -124.21(6) 1_545 2_655
O8 Ca2 O9 P3 115.69(17) . 2_645
O7 Ca2 O9 P3 -164.79(18) . 2_645
O3 Ca2 O9 P3 -84.55(18) . 2_645
O5 Ca2 O9 P3 -11.72(17) . 2_645
O2 Ca2 O9 P3 49.3(3) . 2_645
O6 Ca2 O9 P3 43.55(17) . 2_645
O1 Ca2 O9 P3 170.86(14) . 2_645
O4 Ca2 O9 P3 -78.95(17) . 2_645
P1 Ca2 O9 P3 117.6(3) . 2_645
P2 Ca2 O9 P3 -78.31(16) . 2_645
P3 Ca2 O9 P3 15.81(16) . 2_645
O8 Ca2 O9 Ca3 -39.81(7) . .
O7 Ca2 O9 Ca3 39.71(7) . .
O3 Ca2 O9 Ca3 119.95(9) . .
O5 Ca2 O9 Ca3 -167.22(7) . .
O2 Ca2 O9 Ca3 -106.20(17) . .
O6 Ca2 O9 Ca3 -111.95(8) . .
O1 Ca2 O9 Ca3 15.36(16) . .
O4 Ca2 O9 Ca3 125.55(8) . .
P1 Ca2 O9 Ca3 -37.9(3) . .
P2 Ca2 O9 Ca3 126.19(5) . .
P3 Ca2 O9 Ca3 -139.69(6) . .
O8 Ca2 O9 Ca1 -135.85(8) . 3_675
O7 Ca2 O9 Ca1 -56.33(8) . 3_675
O3 Ca2 O9 Ca1 23.90(12) . 3_675
O5 Ca2 O9 Ca1 96.74(8) . 3_675
O2 Ca2 O9 Ca1 157.76(14) . 3_675
O6 Ca2 O9 Ca1 152.01(8) . 3_675
O1 Ca2 O9 Ca1 -80.68(15) . 3_675
O4 Ca2 O9 Ca1 29.51(7) . 3_675
P1 Ca2 O9 Ca1 -133.9(2) . 3_675
P2 Ca2 O9 Ca1 30.15(7) . 3_675
P3 Ca2 O9 Ca1 124.27(6) . 3_675
O7 Ca3 O9 P3 164.50(17) . 2_645
O8 Ca3 O9 P3 -115.76(17) . 2_645
O2 Ca3 O9 P3 -49.5(3) 1_545 2_645
O3 Ca3 O9 P3 84.26(18) 1_545 2_645
O5 Ca3 O9 P3 11.60(16) 1_545 2_645
O12 Ca3 O9 P3 78.62(17) . 2_645
O10 Ca3 O9 P3 -170.83(14) . 2_645
O11 Ca3 O9 P3 -43.67(16) . 2_645
P3 Ca3 O9 P3 -15.98(16) 1_545 2_645
P2 Ca3 O9 P3 78.11(16) 1_545 2_645
P1 Ca3 O9 P3 -117.9(2) 1_545 2_645
O7 Ca3 O9 Ca2 -39.86(7) . .
O8 Ca3 O9 Ca2 39.88(7) . .
O2 Ca3 O9 Ca2 106.14(17) 1_545 .
O3 Ca3 O9 Ca2 -120.10(9) 1_545 .
O5 Ca3 O9 Ca2 167.23(7) 1_545 .
O12 Ca3 O9 Ca2 -125.74(8) . .
O10 Ca3 O9 Ca2 -15.19(16) . .
O11 Ca3 O9 Ca2 111.97(8) . .
P3 Ca3 O9 Ca2 139.66(6) 1_545 .
P2 Ca3 O9 Ca2 -126.25(5) 1_545 .
P1 Ca3 O9 Ca2 37.7(3) 1_545 .
O7 Ca3 O9 Ca1 56.35(8) . 3_675
O8 Ca3 O9 Ca1 136.10(8) . 3_675
O2 Ca3 O9 Ca1 -157.65(14) 1_545 3_675
O3 Ca3 O9 Ca1 -23.89(12) 1_545 3_675
O5 Ca3 O9 Ca1 -96.55(7) 1_545 3_675
O12 Ca3 O9 Ca1 -29.52(7) . 3_675
O10 Ca3 O9 Ca1 81.02(16) . 3_675
O11 Ca3 O9 Ca1 -151.82(8) . 3_675
P3 Ca3 O9 Ca1 -124.13(6) 1_545 3_675
P2 Ca3 O9 Ca1 -30.03(7) 1_545 3_675
P1 Ca3 O9 Ca1 134.0(2) 1_545 3_675
O7 Ca3 O10 P1 -178.75(15) . 1_545
O9 Ca3 O10 P1 155.71(12) . 1_545
O8 Ca3 O10 P1 101.83(13) . 1_545
O2 Ca3 O10 P1 6.66(10) 1_545 1_545
O3 Ca3 O10 P1 -81.06(13) 1_545 1_545
O5 Ca3 O10 P1 -27.25(16) 1_545 1_545
O12 Ca3 O10 P1 -108.73(13) . 1_545
O11 Ca3 O10 P1 38.11(15) . 1_545
P3 Ca3 O10 P1 5.93(16) 1_545 1_545
P2 Ca3 O10 P1 -91.64(12) 1_545 1_545
O7 Ca3 O10 Ca5 39.77(9) . 1_655
O9 Ca3 O10 Ca5 14.2(2) . 1_655
O8 Ca3 O10 Ca5 -39.65(10) . 1_655
O2 Ca3 O10 Ca5 -134.81(14) 1_545 1_655
O3 Ca3 O10 Ca5 137.47(12) 1_545 1_655
O5 Ca3 O10 Ca5 -168.72(8) 1_545 1_655
O12 Ca3 O10 Ca5 109.79(10) . 1_655
O11 Ca3 O10 Ca5 -103.36(10) . 1_655
P3 Ca3 O10 Ca5 -135.54(7) 1_545 1_655
P2 Ca3 O10 Ca5 126.89(8) 1_545 1_655
P1 Ca3 O10 Ca5 -141.47(19) 1_545 1_655
O7 Ca3 O10 Ca1 -81.85(9) . 1_545
O9 Ca3 O10 Ca1 -107.40(14) . 1_545
O8 Ca3 O10 Ca1 -161.28(10) . 1_545
O2 Ca3 O10 Ca1 103.56(11) 1_545 1_545
O3 Ca3 O10 Ca1 15.84(8) 1_545 1_545
O5 Ca3 O10 Ca1 69.65(11) 1_545 1_545
O12 Ca3 O10 Ca1 -11.84(12) . 1_545
O11 Ca3 O10 Ca1 135.01(9) . 1_545
P3 Ca3 O10 Ca1 102.83(8) 1_545 1_545
P2 Ca3 O10 Ca1 5.26(8) 1_545 1_545
P1 Ca3 O10 Ca1 96.90(14) 1_545 1_545
O7 Ca3 O11 P3 155.97(12) . 1_545
O9 Ca3 O11 P3 101.96(12) . 1_545
O8 Ca3 O11 P3 -178.78(14) . 1_545
O2 Ca3 O11 P3 -81.16(12) 1_545 1_545
O3 Ca3 O11 P3 -27.41(15) 1_545 1_545
O5 Ca3 O11 P3 6.54(10) 1_545 1_545
O12 Ca3 O11 P3 38.09(14) . 1_545
O10 Ca3 O11 P3 -108.79(12) . 1_545
P2 Ca3 O11 P3 5.80(14) 1_545 1_545
P1 Ca3 O11 P3 -91.71(11) 1_545 1_545
O7 Ca3 O11 Ca4 14.61(19) . 2_655
O9 Ca3 O11 Ca4 -39.40(10) . 2_655
O8 Ca3 O11 Ca4 39.86(9) . 2_655
O2 Ca3 O11 Ca4 137.48(12) 1_545 2_655
O3 Ca3 O11 Ca4 -168.77(8) 1_545 2_655
O5 Ca3 O11 Ca4 -134.82(13) 1_545 2_655
O12 Ca3 O11 Ca4 -103.28(10) . 2_655
O10 Ca3 O11 Ca4 109.84(10) . 2_655
P3 Ca3 O11 Ca4 -141.36(17) 1_545 2_655
P2 Ca3 O11 Ca4 -135.56(7) 1_545 2_655
P1 Ca3 O11 Ca4 126.93(8) 1_545 2_655
O7 Ca3 O11 Ca5 -107.13(14) . 2_645
O9 Ca3 O11 Ca5 -161.14(10) . 2_645
O8 Ca3 O11 Ca5 -81.88(9) . 2_645
O2 Ca3 O11 Ca5 15.74(9) 1_545 2_645
O3 Ca3 O11 Ca5 69.49(11) 1_545 2_645
O5 Ca3 O11 Ca5 103.44(12) 1_545 2_645
O12 Ca3 O11 Ca5 134.99(9) . 2_645
O10 Ca3 O11 Ca5 -11.89(12) . 2_645
P3 Ca3 O11 Ca5 96.90(14) 1_545 2_645
P2 Ca3 O11 Ca5 102.70(8) 1_545 2_645
P1 Ca3 O11 Ca5 5.19(8) 1_545 2_645
O5 Ca4 O12 P2 75.95(14) 1_545 1_545
O6 Ca4 O12 P2 165.23(14) 2_645 1_545
O11 Ca4 O12 P2 8.7(2) 2_645 1_545
O4 Ca4 O12 P2 -5.60(8) 1_545 1_545
Cl1B Ca4 O12 P2 -66.86(13) 3_565 1_545
Cl1A Ca4 O12 P2 -117.21(14) 3_565 1_545
O8 Ca4 O12 P2 170.03(9) 2_645 1_545
Cl1A Ca4 O12 P2 -128.72(15) . 1_545
Cl1B Ca4 O12 P2 -56.73(14) 1_545 1_545
P3 Ca4 O12 P2 87.22(12) 1_545 1_545
O5 Ca4 O12 Ca1 -125.01(15) 1_545 3_675
O6 Ca4 O12 Ca1 -35.73(14) 2_645 3_675
O11 Ca4 O12 Ca1 167.74(13) 2_645 3_675
O4 Ca4 O12 Ca1 153.4(2) 1_545 3_675
Cl1B Ca4 O12 Ca1 92.18(13) 3_565 3_675
Cl1A Ca4 O12 Ca1 41.83(12) 3_565 3_675
O8 Ca4 O12 Ca1 -30.9(2) 2_645 3_675
P2 Ca4 O12 Ca1 159.0(2) 1_545 3_675
Cl1A Ca4 O12 Ca1 30.32(11) . 3_675
Cl1B Ca4 O12 Ca1 102.32(13) 1_545 3_675
P3 Ca4 O12 Ca1 -113.74(12) 1_545 3_675
O5 Ca4 O12 Ca3 -16.17(9) 1_545 .
O6 Ca4 O12 Ca3 73.11(9) 2_645 .
O11 Ca4 O12 Ca3 -83.42(16) 2_645 .
O4 Ca4 O12 Ca3 -97.72(12) 1_545 .
Cl1B Ca4 O12 Ca3 -158.98(8) 3_565 .
Cl1A Ca4 O12 Ca3 150.67(10) 3_565 .
O8 Ca4 O12 Ca3 77.92(16) 2_645 .
P2 Ca4 O12 Ca3 -92.12(13) 1_545 .
Cl1A Ca4 O12 Ca3 139.16(10) . .
Cl1B Ca4 O12 Ca3 -148.84(7) 1_545 .
P3 Ca4 O12 Ca3 -4.90(7) 1_545 .
O7 Ca3 O12 P2 101.74(11) . 1_545
O9 Ca3 O12 P2 -178.94(13) . 1_545
O8 Ca3 O12 P2 155.87(11) . 1_545
O2 Ca3 O12 P2 -27.44(13) 1_545 1_545
O3 Ca3 O12 P2 6.55(10) 1_545 1_545
O5 Ca3 O12 P2 -81.10(12) 1_545 1_545
O10 Ca3 O12 P2 38.04(14) . 1_545
O11 Ca3 O12 P2 -108.79(11) . 1_545
P3 Ca3 O12 P2 -91.72(10) 1_545 1_545
P1 Ca3 O12 P2 5.80(13) 1_545 1_545
O7 Ca3 O12 Ca1 -39.57(8) . 3_675
O9 Ca3 O12 Ca1 39.76(8) . 3_675
O8 Ca3 O12 Ca1 14.57(15) . 3_675
O2 Ca3 O12 Ca1 -168.74(7) 1_545 3_675
O3 Ca3 O12 Ca1 -134.76(11) 1_545 3_675
O5 Ca3 O12 Ca1 137.60(10) 1_545 3_675
O10 Ca3 O12 Ca1 -103.26(9) . 3_675
O11 Ca3 O12 Ca1 109.91(9) . 3_675
P3 Ca3 O12 Ca1 126.98(6) 1_545 3_675
P2 Ca3 O12 Ca1 -141.30(14) 1_545 3_675
P1 Ca3 O12 Ca1 -135.51(6) 1_545 3_675
O7 Ca3 O12 Ca4 -161.39(9) . .
O9 Ca3 O12 Ca4 -82.06(8) . .
O8 Ca3 O12 Ca4 -107.25(13) . .
O2 Ca3 O12 Ca4 69.44(10) 1_545 .
O3 Ca3 O12 Ca4 103.42(11) 1_545 .
O5 Ca3 O12 Ca4 15.78(8) 1_545 .
O10 Ca3 O12 Ca4 134.92(8) . .
O11 Ca3 O12 Ca4 -11.91(11) . .
P3 Ca3 O12 Ca4 5.16(7) 1_545 .
P2 Ca3 O12 Ca4 96.88(13) 1_545 .
P1 Ca3 O12 Ca4 102.67(7) 1_545 .
Ca5 O1 P1 O8 19.7(2) 1_655 2_755
Ca1 O1 P1 O8 -132.12(11) . 2_755
Ca2 O1 P1 O8 131.08(11) . 2_755
Ca5 O1 P1 O10 143.5(2) 1_655 1_565
Ca1 O1 P1 O10 -8.34(12) . 1_565
Ca2 O1 P1 O10 -105.13(12) . 1_565
Ca5 O1 P1 O2 -102.2(2) 1_655 .
Ca1 O1 P1 O2 105.95(12) . .
Ca2 O1 P1 O2 9.16(13) . .
Ca5 O1 P1 Ca1 151.9(2) 1_655 .
Ca2 O1 P1 Ca1 -96.79(9) . .
Ca5 O1 P1 Ca2 -111.3(2) 1_655 .
Ca1 O1 P1 Ca2 96.79(9) . .
Ca5 O1 P1 Ca3 -152.12(16) 1_655 1_565
Ca1 O1 P1 Ca3 56.02(9) . 1_565
Ca2 O1 P1 Ca3 -40.77(9) . 1_565
Ca5 O1 P1 Ca5 -67.7(2) 1_655 2_655
Ca1 O1 P1 Ca5 140.48(5) . 2_655
Ca2 O1 P1 Ca5 43.68(11) . 2_655
Ca5 O1 P1 Ca4 66.79(19) 1_655 1_665
Ca1 O1 P1 Ca4 -85.07(6) . 1_665
Ca2 O1 P1 Ca4 178.14(8) . 1_665
Ca5 O2 P1 O8 0.1(2) 2_655 2_755
Ca2 O2 P1 O8 -133.37(14) . 2_755
Ca3 O2 P1 O8 133.46(14) 1_565 2_755
Ca5 O2 P1 O10 -122.52(19) 2_655 1_565
Ca2 O2 P1 O10 103.98(16) . 1_565
Ca3 O2 P1 O10 10.81(17) 1_565 1_565
Ca5 O2 P1 O1 122.61(18) 2_655 .
Ca2 O2 P1 O1 -10.89(16) . .
Ca3 O2 P1 O1 -104.06(15) 1_565 .
Ca5 O2 P1 Ca1 180.00(12) 2_655 .
Ca2 O2 P1 Ca1 46.49(14) . .
Ca3 O2 P1 Ca1 -46.68(14) 1_565 .
Ca5 O2 P1 Ca2 133.5(2) 2_655 .
Ca3 O2 P1 Ca2 -93.17(10) 1_565 .
Ca5 O2 P1 Ca3 -133.3(2) 2_655 1_565
Ca2 O2 P1 Ca3 93.17(10) . 1_565
Ca2 O2 P1 Ca5 -133.5(2) . 2_655
Ca3 O2 P1 Ca5 133.3(2) 1_565 2_655
Ca5 O2 P1 Ca4 0.4(7) 2_655 1_665
Ca2 O2 P1 Ca4 -133.1(5) . 1_665
Ca3 O2 P1 Ca4 133.7(5) 1_565 1_665
O3 Ca1 P1 O8 179.79(19) . 2_755
O4 Ca1 P1 O8 100.68(19) 3_675 2_755
O12 Ca1 P1 O8 -100.91(19) 3_675 2_755
O1 Ca1 P1 O8 84.9(2) . 2_755
O10 Ca1 P1 O8 -85.3(2) 1_565 2_755
Cl1A Ca1 P1 O8 -28.27(19) 3_675 2_755
Cl1B Ca1 P1 O8 27.63(19) 3_675 2_755
Cl1B Ca1 P1 O8 40.05(19) 1_655 2_755
Cl1A Ca1 P1 O8 -39.76(19) 1_665 2_755
P2 Ca1 P1 O8 179.88(18) . 2_755
O3 Ca1 P1 O10 -94.96(14) . 1_565
O4 Ca1 P1 O10 -174.07(14) 3_675 1_565
O12 Ca1 P1 O10 -15.65(13) 3_675 1_565
O1 Ca1 P1 O10 170.18(14) . 1_565
Cl1A Ca1 P1 O10 56.99(13) 3_675 1_565
Cl1B Ca1 P1 O10 112.88(13) 3_675 1_565
Cl1B Ca1 P1 O10 125.30(13) 1_655 1_565
Cl1A Ca1 P1 O10 45.50(13) 1_665 1_565
P2 Ca1 P1 O10 -94.86(12) . 1_565
O3 Ca1 P1 O1 94.86(13) . .
O4 Ca1 P1 O1 15.75(13) 3_675 .
O12 Ca1 P1 O1 174.17(13) 3_675 .
O10 Ca1 P1 O1 -170.18(14) 1_565 .
Cl1A Ca1 P1 O1 -113.20(12) 3_675 .
Cl1B Ca1 P1 O1 -57.30(12) 3_675 .
Cl1B Ca1 P1 O1 -44.88(12) 1_655 .
Cl1A Ca1 P1 O1 -124.68(12) 1_665 .
P2 Ca1 P1 O1 94.95(11) . .
O3 Ca1 P1 O2 -0.02(16) . .
O4 Ca1 P1 O2 -79.14(15) 3_675 .
O12 Ca1 P1 O2 79.28(15) 3_675 .
O1 Ca1 P1 O2 -94.89(17) . .
O10 Ca1 P1 O2 94.93(18) 1_565 .
Cl1A Ca1 P1 O2 151.92(15) 3_675 .
Cl1B Ca1 P1 O2 -152.19(15) 3_675 .
Cl1B Ca1 P1 O2 -139.77(14) 1_655 .
Cl1A Ca1 P1 O2 140.43(14) 1_665 .
P2 Ca1 P1 O2 0.07(14) . .
O3 Ca1 P1 Ca2 32.87(8) . .
O4 Ca1 P1 Ca2 -46.24(7) 3_675 .
O12 Ca1 P1 Ca2 112.17(7) 3_675 .
O1 Ca1 P1 Ca2 -61.99(11) . .
O10 Ca1 P1 Ca2 127.83(12) 1_565 .
Cl1A Ca1 P1 Ca2 -175.19(6) 3_675 .
Cl1B Ca1 P1 Ca2 -119.30(5) 3_675 .
Cl1B Ca1 P1 Ca2 -106.88(5) 1_655 .
Cl1A Ca1 P1 Ca2 173.32(5) 1_665 .
P2 Ca1 P1 Ca2 32.96(3) . .
O3 Ca1 P1 Ca3 -33.10(8) . 1_565
O4 Ca1 P1 Ca3 -112.21(7) 3_675 1_565
O12 Ca1 P1 Ca3 46.21(7) 3_675 1_565
O1 Ca1 P1 Ca3 -127.96(11) . 1_565
O10 Ca1 P1 Ca3 61.86(12) 1_565 1_565
Cl1A Ca1 P1 Ca3 118.84(6) 3_675 1_565
Cl1B Ca1 P1 Ca3 174.74(5) 3_675 1_565
Cl1B Ca1 P1 Ca3 -172.84(5) 1_655 1_565
Cl1A Ca1 P1 Ca3 107.36(5) 1_665 1_565
P2 Ca1 P1 Ca3 -33.01(3) . 1_565
O3 Ca1 P1 Ca5 -0.02(11) . 2_655
O4 Ca1 P1 Ca5 -79.14(10) 3_675 2_655
O12 Ca1 P1 Ca5 79.28(10) 3_675 2_655
O1 Ca1 P1 Ca5 -94.88(13) . 2_655
O10 Ca1 P1 Ca5 94.93(14) 1_565 2_655
Cl1A Ca1 P1 Ca5 151.92(9) 3_675 2_655
Cl1B Ca1 P1 Ca5 -152.19(9) 3_675 2_655
Cl1B Ca1 P1 Ca5 -139.77(8) 1_655 2_655
Cl1A Ca1 P1 Ca5 140.43(9) 1_665 2_655
P2 Ca1 P1 Ca5 0.07(9) . 2_655
O3 Ca1 P1 Ca4 179.89(9) . 1_665
O4 Ca1 P1 Ca4 100.78(7) 3_675 1_665
O12 Ca1 P1 Ca4 -100.81(7) 3_675 1_665
O1 Ca1 P1 Ca4 85.03(11) . 1_665
O10 Ca1 P1 Ca4 -85.16(12) 1_565 1_665
Cl1A Ca1 P1 Ca4 -28.17(6) 3_675 1_665
Cl1B Ca1 P1 Ca4 27.72(5) 3_675 1_665
Cl1B Ca1 P1 Ca4 40.14(5) 1_655 1_665
Cl1A Ca1 P1 Ca4 -39.66(5) 1_665 1_665
P2 Ca1 P1 Ca4 179.98(3) . 1_665
O9 Ca2 P1 O8 -18.3(3) . 2_755
O8 Ca2 P1 O8 -16.36(15) . 2_755
O7 Ca2 P1 O8 -93.15(15) . 2_755
O3 Ca2 P1 O8 -178.93(15) . 2_755
O5 Ca2 P1 O8 110.17(15) . 2_755
O2 Ca2 P1 O8 75.83(19) . 2_755
O6 Ca2 P1 O8 54.39(15) . 2_755
O1 Ca2 P1 O8 -92.16(19) . 2_755
O4 Ca2 P1 O8 -179.59(15) . 2_755
P2 Ca2 P1 O8 177.51(14) . 2_755
P3 Ca2 P1 O8 82.87(14) . 2_755
O9 Ca2 P1 O10 172.6(3) . 1_565
O8 Ca2 P1 O10 174.49(13) . 1_565
O7 Ca2 P1 O10 97.70(13) . 1_565
O3 Ca2 P1 O10 11.92(13) . 1_565
O5 Ca2 P1 O10 -58.98(13) . 1_565
O2 Ca2 P1 O10 -93.31(18) . 1_565
O6 Ca2 P1 O10 -114.76(13) . 1_565
O1 Ca2 P1 O10 98.69(13) . 1_565
O4 Ca2 P1 O10 11.27(14) . 1_565
P2 Ca2 P1 O10 8.37(12) . 1_565
P3 Ca2 P1 O10 -86.27(12) . 1_565
O9 Ca2 P1 O1 73.9(3) . .
O8 Ca2 P1 O1 75.80(13) . .
O7 Ca2 P1 O1 -0.99(13) . .
O3 Ca2 P1 O1 -86.77(13) . .
O5 Ca2 P1 O1 -157.67(13) . .
O2 Ca2 P1 O1 167.99(18) . .
O6 Ca2 P1 O1 146.55(13) . .
O4 Ca2 P1 O1 -87.43(13) . .
P2 Ca2 P1 O1 -90.32(12) . .
P3 Ca2 P1 O1 175.03(12) . .
O9 Ca2 P1 O2 -94.1(3) . .
O8 Ca2 P1 O2 -92.19(15) . .
O7 Ca2 P1 O2 -168.98(14) . .
O3 Ca2 P1 O2 105.24(15) . .
O5 Ca2 P1 O2 34.34(14) . .
O6 Ca2 P1 O2 -21.44(14) . .
O1 Ca2 P1 O2 -167.99(18) . .
O4 Ca2 P1 O2 104.58(14) . .
P2 Ca2 P1 O2 101.68(13) . .
P3 Ca2 P1 O2 7.04(13) . .
O9 Ca2 P1 Ca1 129.1(2) . .
O8 Ca2 P1 Ca1 131.04(6) . .
O7 Ca2 P1 Ca1 54.25(6) . .
O3 Ca2 P1 Ca1 -31.53(6) . .
O5 Ca2 P1 Ca1 -102.43(6) . .
O2 Ca2 P1 Ca1 -136.77(14) . .
O6 Ca2 P1 Ca1 -158.21(6) . .
O1 Ca2 P1 Ca1 55.24(12) . .
O4 Ca2 P1 Ca1 -32.19(7) . .
P2 Ca2 P1 Ca1 -35.09(3) . .
P3 Ca2 P1 Ca1 -129.73(3) . .
O9 Ca2 P1 Ca3 -148.5(2) . 1_565
O8 Ca2 P1 Ca3 -146.57(6) . 1_565
O7 Ca2 P1 Ca3 136.64(7) . 1_565
O3 Ca2 P1 Ca3 50.86(6) . 1_565
O5 Ca2 P1 Ca3 -20.04(5) . 1_565
O2 Ca2 P1 Ca3 -54.38(13) . 1_565
O6 Ca2 P1 Ca3 -75.82(6) . 1_565
O1 Ca2 P1 Ca3 137.63(12) . 1_565
O4 Ca2 P1 Ca3 50.20(7) . 1_565
P2 Ca2 P1 Ca3 47.31(2) . 1_565
P3 Ca2 P1 Ca3 -47.34(2) . 1_565
O9 Ca2 P1 Ca5 -68.6(2) . 2_655
O8 Ca2 P1 Ca5 -66.74(6) . 2_655
O7 Ca2 P1 Ca5 -143.53(6) . 2_655
O3 Ca2 P1 Ca5 130.69(7) . 2_655
O5 Ca2 P1 Ca5 59.79(5) . 2_655
O2 Ca2 P1 Ca5 25.45(13) . 2_655
O6 Ca2 P1 Ca5 4.01(6) . 2_655
O1 Ca2 P1 Ca5 -142.55(12) . 2_655
O4 Ca2 P1 Ca5 130.03(7) . 2_655
P2 Ca2 P1 Ca5 127.13(3) . 2_655
P3 Ca2 P1 Ca5 32.49(3) . 2_655
O9 Ca2 P1 Ca4 71.0(3) . 1_665
O8 Ca2 P1 Ca4 72.90(7) . 1_665
O7 Ca2 P1 Ca4 -3.89(8) . 1_665
O3 Ca2 P1 Ca4 -89.67(8) . 1_665
O5 Ca2 P1 Ca4 -160.57(6) . 1_665
O2 Ca2 P1 Ca4 165.09(14) . 1_665
O6 Ca2 P1 Ca4 143.65(7) . 1_665
O1 Ca2 P1 Ca4 -2.90(12) . 1_665
O4 Ca2 P1 Ca4 -90.33(8) . 1_665
P2 Ca2 P1 Ca4 -93.23(5) . 1_665
P3 Ca2 P1 Ca4 172.13(4) . 1_665
Ca1 O4 P2 O7 19.8(3) 3_675 3_675
Ca4 O4 P2 O7 -132.07(11) 1_565 3_675
Ca2 O4 P2 O7 131.26(11) . 3_675
Ca1 O4 P2 O12 143.5(3) 3_675 1_565
Ca4 O4 P2 O12 -8.31(12) 1_565 1_565
Ca2 O4 P2 O12 -104.98(12) . 1_565
Ca1 O4 P2 O3 -102.2(3) 3_675 .
Ca4 O4 P2 O3 105.96(12) 1_565 .
Ca2 O4 P2 O3 9.28(12) . .
Ca1 O4 P2 Ca4 151.8(3) 3_675 1_565
Ca2 O4 P2 Ca4 -96.67(10) . 1_565
Ca1 O4 P2 Ca2 -111.5(3) 3_675 .
Ca4 O4 P2 Ca2 96.67(10) 1_565 .
Ca1 O4 P2 Ca3 -152.1(2) 3_675 1_565
Ca4 O4 P2 Ca3 56.02(12) 1_565 1_565
Ca2 O4 P2 Ca3 -40.66(9) . 1_565
Ca1 O4 P2 Ca1 -67.7(3) 3_675 .
Ca4 O4 P2 Ca1 140.51(6) 1_565 .
Ca2 O4 P2 Ca1 43.84(10) . .
Ca1 O4 P2 Ca5 66.8(2) 3_675 3_575
Ca4 O4 P2 Ca5 -85.08(8) 1_565 3_575
Ca2 O4 P2 Ca5 178.25(7) . 3_575
Ca1 O3 P2 O4 122.59(18) . .
Ca2 O3 P2 O4 -11.07(15) . .
Ca3 O3 P2 O4 -104.33(14) 1_565 .
Ca1 O3 P2 O7 0.1(3) . 3_675
Ca2 O3 P2 O7 -133.61(14) . 3_675
Ca3 O3 P2 O7 133.13(14) 1_565 3_675
Ca1 O3 P2 O12 -122.46(18) . 1_565
Ca2 O3 P2 O12 103.88(14) . 1_565
Ca3 O3 P2 O12 10.62(16) 1_565 1_565
Ca1 O3 P2 Ca4 -179.88(12) . 1_565
Ca2 O3 P2 Ca4 46.46(14) . 1_565
Ca3 O3 P2 Ca4 -46.80(14) 1_565 1_565
Ca1 O3 P2 Ca2 133.7(2) . .
Ca3 O3 P2 Ca2 -93.26(9) 1_565 .
Ca1 O3 P2 Ca3 -133.1(2) . 1_565
Ca2 O3 P2 Ca3 93.26(9) . 1_565
Ca2 O3 P2 Ca1 -133.7(2) . .
Ca3 O3 P2 Ca1 133.1(2) 1_565 .
Ca1 O3 P2 Ca5 0.6(7) . 3_575
Ca2 O3 P2 Ca5 -133.0(5) . 3_575
Ca3 O3 P2 Ca5 133.7(5) 1_565 3_575
O9 Ca2 P2 O4 -1.28(12) . .
O8 Ca2 P2 O4 73.5(3) . .
O7 Ca2 P2 O4 75.60(12) . .
O3 Ca2 P2 O4 167.80(17) . .
O5 Ca2 P2 O4 -86.90(12) . .
O2 Ca2 P2 O4 -157.74(11) . .
O6 Ca2 P2 O4 -87.58(13) . .
O1 Ca2 P2 O4 146.33(12) . .
P1 Ca2 P2 O4 174.87(11) . .
P3 Ca2 P2 O4 -90.52(11) . .
O9 Ca2 P2 O7 -93.51(15) . 3_675
O8 Ca2 P2 O7 -18.7(3) . 3_675
O7 Ca2 P2 O7 -16.62(19) . 3_675
O3 Ca2 P2 O7 75.58(18) . 3_675
O5 Ca2 P2 O7 -179.13(16) . 3_675
O2 Ca2 P2 O7 110.03(15) . 3_675
O6 Ca2 P2 O7 -179.81(15) . 3_675
O1 Ca2 P2 O7 54.10(15) . 3_675
O4 Ca2 P2 O7 -92.23(18) . 3_675
P1 Ca2 P2 O7 82.65(15) . 3_675
P3 Ca2 P2 O7 177.25(14) . 3_675
O9 Ca2 P2 O12 97.60(13) . 1_565
O8 Ca2 P2 O12 172.4(3) . 1_565
O7 Ca2 P2 O12 174.49(12) . 1_565
O3 Ca2 P2 O12 -93.31(18) . 1_565
O5 Ca2 P2 O12 11.98(13) . 1_565
O2 Ca2 P2 O12 -58.86(12) . 1_565
O6 Ca2 P2 O12 11.30(14) . 1_565
O1 Ca2 P2 O12 -114.79(13) . 1_565
O4 Ca2 P2 O12 98.88(13) . 1_565
P1 Ca2 P2 O12 -86.24(11) . 1_565
P3 Ca2 P2 O12 8.36(12) . 1_565
O9 Ca2 P2 O3 -169.08(14) . .
O8 Ca2 P2 O3 -94.3(3) . .
O7 Ca2 P2 O3 -92.20(14) . .
O5 Ca2 P2 O3 105.30(15) . .
O2 Ca2 P2 O3 34.45(14) . .
O6 Ca2 P2 O3 104.61(14) . .
O1 Ca2 P2 O3 -21.48(14) . .
O4 Ca2 P2 O3 -167.80(17) . .
P1 Ca2 P2 O3 7.07(13) . .
P3 Ca2 P2 O3 101.68(13) . .
O9 Ca2 P2 Ca4 54.13(6) . 1_565
O8 Ca2 P2 Ca4 128.9(3) . 1_565
O7 Ca2 P2 Ca4 131.02(6) . 1_565
O3 Ca2 P2 Ca4 -136.78(13) . 1_565
O5 Ca2 P2 Ca4 -31.49(7) . 1_565
O2 Ca2 P2 Ca4 -102.33(5) . 1_565
O6 Ca2 P2 Ca4 -32.17(7) . 1_565
O1 Ca2 P2 Ca4 -158.26(6) . 1_565
O4 Ca2 P2 Ca4 55.41(10) . 1_565
P1 Ca2 P2 Ca4 -129.71(3) . 1_565
P3 Ca2 P2 Ca4 -35.11(3) . 1_565
O9 Ca2 P2 Ca3 136.53(6) . 1_565
O8 Ca2 P2 Ca3 -148.7(3) . 1_565
O7 Ca2 P2 Ca3 -146.59(6) . 1_565
O3 Ca2 P2 Ca3 -54.39(13) . 1_565
O5 Ca2 P2 Ca3 50.91(6) . 1_565
O2 Ca2 P2 Ca3 -19.93(5) . 1_565
O6 Ca2 P2 Ca3 50.23(7) . 1_565
O1 Ca2 P2 Ca3 -75.86(6) . 1_565
O4 Ca2 P2 Ca3 137.81(11) . 1_565
P1 Ca2 P2 Ca3 -47.32(2) . 1_565
P3 Ca2 P2 Ca3 47.29(2) . 1_565
O9 Ca2 P2 Ca1 -143.68(6) . .
O8 Ca2 P2 Ca1 -68.9(3) . .
O7 Ca2 P2 Ca1 -66.79(6) . .
O3 Ca2 P2 Ca1 25.41(13) . .
O5 Ca2 P2 Ca1 130.70(7) . .
O2 Ca2 P2 Ca1 59.86(5) . .
O6 Ca2 P2 Ca1 130.02(7) . .
O1 Ca2 P2 Ca1 3.93(6) . .
O4 Ca2 P2 Ca1 -142.40(11) . .
P1 Ca2 P2 Ca1 32.48(3) . .
P3 Ca2 P2 Ca1 127.08(3) . .
O9 Ca2 P2 Ca5 -4.02(8) . 3_575
O8 Ca2 P2 Ca5 70.7(3) . 3_575
O7 Ca2 P2 Ca5 72.86(7) . 3_575
O3 Ca2 P2 Ca5 165.06(14) . 3_575
O5 Ca2 P2 Ca5 -89.64(8) . 3_575
O2 Ca2 P2 Ca5 -160.48(6) . 3_575
O6 Ca2 P2 Ca5 -90.32(8) . 3_575
O1 Ca2 P2 Ca5 143.59(7) . 3_575
O4 Ca2 P2 Ca5 -2.74(10) . 3_575
P1 Ca2 P2 Ca5 172.13(4) . 3_575
P3 Ca2 P2 Ca5 -93.26(5) . 3_575
O3 Ca1 P2 O4 -72.1(2) . .
O4 Ca1 P2 O4 37.88(18) 3_675 .
O12 Ca1 P2 O4 177.29(16) 3_675 .
O1 Ca1 P2 O4 -43.12(13) . .
O10 Ca1 P2 O4 -101.53(13) 1_565 .
Cl1A Ca1 P2 O4 -155.58(18) 3_675 .
Cl1B Ca1 P2 O4 12.59(19) 3_675 .
O9 Ca1 P2 O4 107.55(13) 3_675 .
P1 Ca1 P2 O4 -72.37(12) . .
Cl1B Ca1 P2 O4 13.34(15) 1_655 .
Cl1A Ca1 P2 O4 -159.14(14) 1_665 .
O3 Ca1 P2 O7 -179.9(3) . 3_675
O4 Ca1 P2 O7 -69.93(14) 3_675 3_675
O12 Ca1 P2 O7 69.49(14) 3_675 3_675
O1 Ca1 P2 O7 -150.93(13) . 3_675
O10 Ca1 P2 O7 150.67(14) 1_565 3_675
Cl1A Ca1 P2 O7 96.61(18) 3_675 3_675
Cl1B Ca1 P2 O7 -95.22(19) 3_675 3_675
O9 Ca1 P2 O7 -0.26(13) 3_675 3_675
P1 Ca1 P2 O7 179.83(12) . 3_675
Cl1B Ca1 P2 O7 -94.46(15) 1_655 3_675
Cl1A Ca1 P2 O7 93.06(15) 1_665 3_675
O3 Ca1 P2 O12 72.3(2) . 1_565
O4 Ca1 P2 O12 -177.68(16) 3_675 1_565
O12 Ca1 P2 O12 -38.26(18) 3_675 1_565
O1 Ca1 P2 O12 101.33(14) . 1_565
O10 Ca1 P2 O12 42.92(14) 1_565 1_565
Cl1A Ca1 P2 O12 -11.13(19) 3_675 1_565
Cl1B Ca1 P2 O12 157.04(18) 3_675 1_565
O9 Ca1 P2 O12 -108.00(13) 3_675 1_565
P1 Ca1 P2 O12 72.08(12) . 1_565
Cl1B Ca1 P2 O12 157.79(15) 1_655 1_565
Cl1A Ca1 P2 O12 -14.69(15) 1_665 1_565
O4 Ca1 P2 O3 110.0(2) 3_675 .
O12 Ca1 P2 O3 -110.6(2) 3_675 .
O1 Ca1 P2 O3 29.0(2) . .
O10 Ca1 P2 O3 -29.4(2) 1_565 .
Cl1A Ca1 P2 O3 -83.4(3) 3_675 .
Cl1B Ca1 P2 O3 84.7(3) 3_675 .
O9 Ca1 P2 O3 179.7(2) 3_675 .
P1 Ca1 P2 O3 -0.2(2) . .
Cl1B Ca1 P2 O3 85.5(2) 1_655 .
Cl1A Ca1 P2 O3 -87.0(2) 1_665 .
O3 Ca1 P2 Ca4 0.2(2) . 1_565
O4 Ca1 P2 Ca4 110.23(10) 3_675 1_565
O12 Ca1 P2 Ca4 -110.36(10) 3_675 1_565
O1 Ca1 P2 Ca4 29.23(10) . 1_565
O10 Ca1 P2 Ca4 -29.17(10) 1_565 1_565
Cl1A Ca1 P2 Ca4 -83.23(16) 3_675 1_565
Cl1B Ca1 P2 Ca4 84.94(16) 3_675 1_565
O9 Ca1 P2 Ca4 179.90(9) 3_675 1_565
P1 Ca1 P2 Ca4 -0.02(8) . 1_565
Cl1B Ca1 P2 Ca4 85.69(12) 1_655 1_565
Cl1A Ca1 P2 Ca4 -86.79(12) 1_665 1_565
O3 Ca1 P2 Ca2 -33.4(2) . .
O4 Ca1 P2 Ca2 76.66(7) 3_675 .
O12 Ca1 P2 Ca2 -143.92(7) 3_675 .
O1 Ca1 P2 Ca2 -4.34(6) . .
O10 Ca1 P2 Ca2 -62.74(7) 1_565 .
Cl1A Ca1 P2 Ca2 -116.80(13) 3_675 .
Cl1B Ca1 P2 Ca2 51.37(14) 3_675 .
O9 Ca1 P2 Ca2 146.33(6) 3_675 .
P1 Ca1 P2 Ca2 -33.59(3) . .
Cl1B Ca1 P2 Ca2 52.12(9) 1_655 .
Cl1A Ca1 P2 Ca2 -120.35(9) 1_665 .
O3 Ca1 P2 Ca3 33.9(2) . 1_565
O4 Ca1 P2 Ca3 143.88(7) 3_675 1_565
O12 Ca1 P2 Ca3 -76.70(7) 3_675 1_565
O1 Ca1 P2 Ca3 62.88(6) . 1_565
O10 Ca1 P2 Ca3 4.48(7) 1_565 1_565
Cl1A Ca1 P2 Ca3 -49.58(14) 3_675 1_565
Cl1B Ca1 P2 Ca3 118.59(14) 3_675 1_565
O9 Ca1 P2 Ca3 -146.45(6) 3_675 1_565
P1 Ca1 P2 Ca3 33.64(3) . 1_565
Cl1B Ca1 P2 Ca3 119.34(9) 1_655 1_565
Cl1A Ca1 P2 Ca3 -53.13(9) 1_665 1_565
O3 Ca1 P2 Ca5 -179.8(2) . 3_575
O4 Ca1 P2 Ca5 -69.79(8) 3_675 3_575
O12 Ca1 P2 Ca5 69.63(8) 3_675 3_575
O1 Ca1 P2 Ca5 -150.79(7) . 3_575
O10 Ca1 P2 Ca5 150.81(8) 1_565 3_575
Cl1A Ca1 P2 Ca5 96.75(14) 3_675 3_575
Cl1B Ca1 P2 Ca5 -95.08(15) 3_675 3_575
O9 Ca1 P2 Ca5 -0.12(8) 3_675 3_575
P1 Ca1 P2 Ca5 179.96(5) . 3_575
Cl1B Ca1 P2 Ca5 -94.33(10) 1_655 3_575
Cl1A Ca1 P2 Ca5 93.20(10) 1_665 3_575
Ca4 O6 P3 O11 143.2(3) 2_655 1_565
Ca5 O6 P3 O11 -8.33(12) 2_655 1_565
Ca2 O6 P3 O11 -105.07(11) . 1_565
Ca4 O6 P3 O9 19.4(3) 2_655 2_655
Ca5 O6 P3 O9 -132.14(11) 2_655 2_655
Ca2 O6 P3 O9 131.13(11) . 2_655
Ca4 O6 P3 O5 -102.3(2) 2_655 .
Ca5 O6 P3 O5 106.18(12) 2_655 .
Ca2 O6 P3 O5 9.44(12) . .
Ca4 O6 P3 Ca5 151.5(3) 2_655 2_655
Ca2 O6 P3 Ca5 -96.73(8) . 2_655
Ca4 O6 P3 Ca3 -152.27(19) 2_655 1_565
Ca5 O6 P3 Ca3 56.18(10) 2_655 1_565
Ca2 O6 P3 Ca3 -40.55(10) . 1_565
Ca4 O6 P3 Ca2 -111.7(3) 2_655 .
Ca5 O6 P3 Ca2 96.73(8) 2_655 .
Ca4 O6 P3 Ca4 -67.9(2) 2_655 1_565
Ca5 O6 P3 Ca4 140.57(6) 2_655 1_565
Ca2 O6 P3 Ca4 43.84(10) . 1_565
Ca4 O6 P3 Ca1 66.5(2) 2_655 4_586
Ca5 O6 P3 Ca1 -85.05(7) 2_655 4_586
Ca2 O6 P3 Ca1 178.22(7) . 4_586
Ca4 O5 P3 O11 -122.31(19) 1_565 1_565
Ca2 O5 P3 O11 103.82(14) . 1_565
Ca3 O5 P3 O11 10.64(16) 1_565 1_565
Ca4 O5 P3 O6 122.62(19) 1_565 .
Ca2 O5 P3 O6 -11.25(15) . .
Ca3 O5 P3 O6 -104.43(14) 1_565 .
Ca4 O5 P3 O9 0.3(2) 1_565 2_655
Ca2 O5 P3 O9 -133.61(14) . 2_655
Ca3 O5 P3 O9 133.21(15) 1_565 2_655
Ca4 O5 P3 Ca5 -179.87(13) 1_565 2_655
Ca2 O5 P3 Ca5 46.27(14) . 2_655
Ca3 O5 P3 Ca5 -46.91(14) 1_565 2_655
Ca4 O5 P3 Ca3 -133.0(3) 1_565 1_565
Ca2 O5 P3 Ca3 93.18(9) . 1_565
Ca4 O5 P3 Ca2 133.9(3) 1_565 .
Ca3 O5 P3 Ca2 -93.18(9) 1_565 .
Ca2 O5 P3 Ca4 -133.9(3) . 1_565
Ca3 O5 P3 Ca4 133.0(3) 1_565 1_565
Ca4 O5 P3 Ca1 1.5(7) 1_565 4_586
Ca2 O5 P3 Ca1 -132.4(5) . 4_586
Ca3 O5 P3 Ca1 134.5(5) 1_565 4_586
O9 Ca2 P3 O11 174.49(15) . 1_565
O8 Ca2 P3 O11 97.58(15) . 1_565
O7 Ca2 P3 O11 172.1(3) . 1_565
O3 Ca2 P3 O11 -58.98(15) . 1_565
O5 Ca2 P3 O11 -93.55(19) . 1_565
O2 Ca2 P3 O11 11.86(15) . 1_565
O6 Ca2 P3 O11 98.87(13) . 1_565
O1 Ca2 P3 O11 11.13(16) . 1_565
O4 Ca2 P3 O11 -114.85(14) . 1_565
P1 Ca2 P3 O11 8.32(14) . 1_565
P2 Ca2 P3 O11 -86.34(14) . 1_565
O9 Ca2 P3 O6 75.62(13) . .
O8 Ca2 P3 O6 -1.29(12) . .
O7 Ca2 P3 O6 73.2(3) . .
O3 Ca2 P3 O6 -157.85(12) . .
O5 Ca2 P3 O6 167.57(17) . .
O2 Ca2 P3 O6 -87.01(13) . .
O1 Ca2 P3 O6 -87.74(13) . .
O4 Ca2 P3 O6 146.28(12) . .
P1 Ca2 P3 O6 -90.55(11) . .
P2 Ca2 P3 O6 174.79(11) . .
O9 Ca2 P3 O9 -16.58(15) . 2_655
O8 Ca2 P3 O9 -93.48(15) . 2_655
O7 Ca2 P3 O9 -19.0(3) . 2_655
O3 Ca2 P3 O9 109.96(15) . 2_655
O5 Ca2 P3 O9 75.4(2) . 2_655
O2 Ca2 P3 O9 -179.20(15) . 2_655
O6 Ca2 P3 O9 -92.19(19) . 2_655
O1 Ca2 P3 O9 -179.94(15) . 2_655
O4 Ca2 P3 O9 54.09(15) . 2_655
P1 Ca2 P3 O9 177.25(14) . 2_655
P2 Ca2 P3 O9 82.60(14) . 2_655
O9 Ca2 P3 O5 -91.96(15) . .
O8 Ca2 P3 O5 -168.86(14) . .
O7 Ca2 P3 O5 -94.4(3) . .
O3 Ca2 P3 O5 34.58(14) . .
O2 Ca2 P3 O5 105.42(15) . .
O6 Ca2 P3 O5 -167.57(17) . .
O1 Ca2 P3 O5 104.68(14) . .
O4 Ca2 P3 O5 -21.29(14) . .
P1 Ca2 P3 O5 101.87(13) . .
P2 Ca2 P3 O5 7.22(13) . .
O9 Ca2 P3 Ca5 131.05(6) . 2_655
O8 Ca2 P3 Ca5 54.15(6) . 2_655
O7 Ca2 P3 Ca5 128.6(3) . 2_655
O3 Ca2 P3 Ca5 -102.41(6) . 2_655
O5 Ca2 P3 Ca5 -136.99(13) . 2_655
O2 Ca2 P3 Ca5 -31.57(7) . 2_655
O6 Ca2 P3 Ca5 55.44(11) . 2_655
O1 Ca2 P3 Ca5 -32.31(8) . 2_655
O4 Ca2 P3 Ca5 -158.28(6) . 2_655
P1 Ca2 P3 Ca5 -35.11(3) . 2_655
P2 Ca2 P3 Ca5 -129.77(3) . 2_655
O9 Ca2 P3 Ca3 -146.48(7) . 1_565
O8 Ca2 P3 Ca3 136.62(7) . 1_565
O7 Ca2 P3 Ca3 -148.9(3) . 1_565
O3 Ca2 P3 Ca3 -19.94(5) . 1_565
O5 Ca2 P3 Ca3 -54.52(13) . 1_565
O2 Ca2 P3 Ca3 50.90(7) . 1_565
O6 Ca2 P3 Ca3 137.91(12) . 1_565
O1 Ca2 P3 Ca3 50.16(7) . 1_565
O4 Ca2 P3 Ca3 -75.81(6) . 1_565
P1 Ca2 P3 Ca3 47.35(3) . 1_565
P2 Ca2 P3 Ca3 -47.30(3) . 1_565
O9 Ca2 P3 Ca4 -66.70(6) . 1_565
O8 Ca2 P3 Ca4 -143.61(6) . 1_565
O7 Ca2 P3 Ca4 -69.1(3) . 1_565
O3 Ca2 P3 Ca4 59.84(6) . 1_565
O5 Ca2 P3 Ca4 25.26(13) . 1_565
O2 Ca2 P3 Ca4 130.68(7) . 1_565
O6 Ca2 P3 Ca4 -142.32(11) . 1_565
O1 Ca2 P3 Ca4 129.94(7) . 1_565
O4 Ca2 P3 Ca4 3.96(5) . 1_565
P1 Ca2 P3 Ca4 127.13(3) . 1_565
P2 Ca2 P3 Ca4 32.48(3) . 1_565
O9 Ca2 P3 Ca1 72.84(8) . 4_586
O8 Ca2 P3 Ca1 -4.07(8) . 4_586
O7 Ca2 P3 Ca1 70.4(3) . 4_586
O3 Ca2 P3 Ca1 -160.63(6) . 4_586
O5 Ca2 P3 Ca1 164.80(14) . 4_586
O2 Ca2 P3 Ca1 -89.79(8) . 4_586
O6 Ca2 P3 Ca1 -2.78(11) . 4_586
O1 Ca2 P3 Ca1 -90.52(8) . 4_586
O4 Ca2 P3 Ca1 143.50(6) . 4_586
P1 Ca2 P3 Ca1 -93.33(5) . 4_586
P2 Ca2 P3 Ca1 172.01(4) . 4_586
O2 Ca5 Cl1A Cl1A 48.1(6) 2_645 3_565
O10 Ca5 Cl1A Cl1A -18.1(5) 1_455 3_565
O1 Ca5 Cl1A Cl1A -153.9(5) 1_455 3_565
O11 Ca5 Cl1A Cl1A 121.3(5) 2_655 3_565
O6 Ca5 Cl1A Cl1A 68.5(5) 2_645 3_565
Cl1B Ca5 Cl1A Cl1A -178.0(6) . 3_565
O7 Ca5 Cl1A Cl1A -83.2(5) 1_455 3_565
P3 Ca5 Cl1A Cl1A 94.5(5) 2_645 3_565
Cl1B Ca5 Cl1A Cl1A -178.4(5) 3_575 3_565
P1 Ca5 Cl1A Cl1A 8.9(7) 2_645 3_565
O2 Ca5 Cl1A Ca1 -82.43(14) 2_645 3_675
O10 Ca5 Cl1A Ca1 -148.63(11) 1_455 3_675
O1 Ca5 Cl1A Ca1 75.61(13) 1_455 3_675
O11 Ca5 Cl1A Ca1 -9.16(10) 2_655 3_675
O6 Ca5 Cl1A Ca1 -62.02(9) 2_645 3_675
Cl1B Ca5 Cl1A Ca1 51.54(9) . 3_675
O7 Ca5 Cl1A Ca1 146.29(8) 1_455 3_675
P3 Ca5 Cl1A Ca1 -36.03(7) 2_645 3_675
Cl1A Ca5 Cl1A Ca1 -130.5(6) 3_565 3_675
Cl1B Ca5 Cl1A Ca1 51.11(9) 3_575 3_675
P1 Ca5 Cl1A Ca1 -121.63(10) 2_645 3_675
O2 Ca5 Cl1A Ca4 174.88(11) 2_645 3_565
O10 Ca5 Cl1A Ca4 108.68(10) 1_455 3_565
O1 Ca5 Cl1A Ca4 -27.07(13) 1_455 3_565
O11 Ca5 Cl1A Ca4 -111.85(9) 2_655 3_565
O6 Ca5 Cl1A Ca4 -164.71(10) 2_645 3_565
Cl1B Ca5 Cl1A Ca4 -51.14(9) . 3_565
O7 Ca5 Cl1A Ca4 43.60(9) 1_455 3_565
P3 Ca5 Cl1A Ca4 -138.71(7) 2_645 3_565
Cl1A Ca5 Cl1A Ca4 126.8(6) 3_565 3_565
Cl1B Ca5 Cl1A Ca4 -51.58(8) 3_575 3_565
P1 Ca5 Cl1A Ca4 135.69(9) 2_645 3_565
O2 Ca5 Cl1A Ca5 48.1(6) 2_645 3_565
O10 Ca5 Cl1A Ca5 -18.1(5) 1_455 3_565
O1 Ca5 Cl1A Ca5 -153.9(5) 1_455 3_565
O11 Ca5 Cl1A Ca5 121.3(5) 2_655 3_565
O6 Ca5 Cl1A Ca5 68.5(5) 2_645 3_565
Cl1B Ca5 Cl1A Ca5 -178.0(6) . 3_565
O7 Ca5 Cl1A Ca5 -83.2(5) 1_455 3_565
P3 Ca5 Cl1A Ca5 94.5(5) 2_645 3_565
Cl1A Ca5 Cl1A Ca5 0 3_565 3_565
Cl1B Ca5 Cl1A Ca5 -178.4(5) 3_575 3_565
P1 Ca5 Cl1A Ca5 8.9(7) 2_645 3_565
O2 Ca5 Cl1A Ca4 4.88(16) 2_645 .
O10 Ca5 Cl1A Ca4 -61.32(8) 1_455 .
O1 Ca5 Cl1A Ca4 162.93(9) 1_455 .
O11 Ca5 Cl1A Ca4 78.15(8) 2_655 .
O6 Ca5 Cl1A Ca4 25.29(7) 2_645 .
Cl1B Ca5 Cl1A Ca4 138.86(14) . .
O7 Ca5 Cl1A Ca4 -126.39(7) 1_455 .
P3 Ca5 Cl1A Ca4 51.29(5) 2_645 .
Cl1A Ca5 Cl1A Ca4 -43.2(5) 3_565 .
Cl1B Ca5 Cl1A Ca4 138.42(7) 3_575 .
P1 Ca5 Cl1A Ca4 -34.31(17) 2_645 .
O2 Ca5 Cl1A Ca1 88.11(15) 2_645 1_445
O10 Ca5 Cl1A Ca1 21.91(8) 1_455 1_445
O1 Ca5 Cl1A Ca1 -113.85(9) 1_455 1_445
O11 Ca5 Cl1A Ca1 161.37(8) 2_655 1_445
O6 Ca5 Cl1A Ca1 108.51(8) 2_645 1_445
Cl1B Ca5 Cl1A Ca1 -137.92(15) . 1_445
O7 Ca5 Cl1A Ca1 -43.17(8) 1_455 1_445
P3 Ca5 Cl1A Ca1 134.51(6) 2_645 1_445
Cl1A Ca5 Cl1A Ca1 40.0(5) 3_565 1_445
Cl1B Ca5 Cl1A Ca1 -138.35(6) 3_575 1_445
P1 Ca5 Cl1A Ca1 48.91(17) 2_645 1_445
O5 Ca4 Cl1A Cl1A 148.2(4) 1_545 3_565
O6 Ca4 Cl1A Cl1A -152.9(5) 2_645 3_565
O11 Ca4 Cl1A Cl1A -23.7(5) 2_645 3_565
O12 Ca4 Cl1A Cl1A 114.3(5) . 3_565
O4 Ca4 Cl1A Cl1A 67.7(5) 1_545 3_565
Cl1B Ca4 Cl1A Cl1A 6.0(5) 3_565 3_565
O8 Ca4 Cl1A Cl1A -91.3(5) 2_645 3_565
P2 Ca4 Cl1A Cl1A 91.8(5) 1_545 3_565
Cl1B Ca4 Cl1A Cl1A 5.0(4) 1_545 3_565
P3 Ca4 Cl1A Cl1A -179.9(4) 1_545 3_565
O5 Ca4 Cl1A Ca1 12.25(13) 1_545 3_675
O6 Ca4 Cl1A Ca1 71.15(8) 2_645 3_675
O11 Ca4 Cl1A Ca1 -159.71(10) 2_645 3_675
O12 Ca4 Cl1A Ca1 -21.67(8) . 3_675
O4 Ca4 Cl1A Ca1 -68.30(9) 1_545 3_675
Cl1B Ca4 Cl1A Ca1 -129.95(8) 3_565 3_675
Cl1A Ca4 Cl1A Ca1 -136.0(5) 3_565 3_675
O8 Ca4 Cl1A Ca1 132.69(7) 2_645 3_675
P2 Ca4 Cl1A Ca1 -44.16(6) 1_545 3_675
Cl1B Ca4 Cl1A Ca1 -131.02(8) 1_545 3_675
P3 Ca4 Cl1A Ca1 44.09(11) 1_545 3_675
O5 Ca4 Cl1A Ca4 148.2(4) 1_545 3_565
O6 Ca4 Cl1A Ca4 -152.9(5) 2_645 3_565
O11 Ca4 Cl1A Ca4 -23.7(5) 2_645 3_565
O12 Ca4 Cl1A Ca4 114.3(5) . 3_565
O4 Ca4 Cl1A Ca4 67.7(5) 1_545 3_565
Cl1B Ca4 Cl1A Ca4 6.0(5) 3_565 3_565
Cl1A Ca4 Cl1A Ca4 0 3_565 3_565
O8 Ca4 Cl1A Ca4 -91.3(5) 2_645 3_565
P2 Ca4 Cl1A Ca4 91.8(5) 1_545 3_565
Cl1B Ca4 Cl1A Ca4 5.0(4) 1_545 3_565
P3 Ca4 Cl1A Ca4 -179.9(4) 1_545 3_565
O5 Ca4 Cl1A Ca5 -87.78(10) 1_545 .
O6 Ca4 Cl1A Ca5 -28.88(7) 2_645 .
O11 Ca4 Cl1A Ca5 100.26(13) 2_645 .
O12 Ca4 Cl1A Ca5 -121.70(10) . .
O4 Ca4 Cl1A Ca5 -168.34(8) 1_545 .
Cl1B Ca4 Cl1A Ca5 130.02(7) 3_565 .
Cl1A Ca4 Cl1A Ca5 124.0(5) 3_565 .
O8 Ca4 Cl1A Ca5 32.66(8) 2_645 .
P2 Ca4 Cl1A Ca5 -144.19(6) 1_545 .
Cl1B Ca4 Cl1A Ca5 128.95(8) 1_545 .
P3 Ca4 Cl1A Ca5 -55.95(9) 1_545 .
O5 Ca4 Cl1A Ca5 100.87(11) 1_545 3_565
O6 Ca4 Cl1A Ca5 159.77(9) 2_645 3_565
O11 Ca4 Cl1A Ca5 -71.09(12) 2_645 3_565
O12 Ca4 Cl1A Ca5 66.95(8) . 3_565
O4 Ca4 Cl1A Ca5 20.32(8) 1_545 3_565
Cl1B Ca4 Cl1A Ca5 -41.33(7) 3_565 3_565
Cl1A Ca4 Cl1A Ca5 -47.4(4) 3_565 3_565
O8 Ca4 Cl1A Ca5 -138.69(6) 2_645 3_565
P2 Ca4 Cl1A Ca5 44.46(4) 1_545 3_565
Cl1B Ca4 Cl1A Ca5 -42.40(5) 1_545 3_565
P3 Ca4 Cl1A Ca5 132.71(5) 1_545 3_565
O5 Ca4 Cl1A Ca1 -174.91(8) 1_545 1_445
O6 Ca4 Cl1A Ca1 -116.01(8) 2_645 1_445
O11 Ca4 Cl1A Ca1 13.13(14) 2_645 1_445
O12 Ca4 Cl1A Ca1 151.17(10) . 1_445
O4 Ca4 Cl1A Ca1 104.54(7) 1_545 1_445
Cl1B Ca4 Cl1A Ca1 42.89(7) 3_565 1_445
Cl1A Ca4 Cl1A Ca1 36.8(4) 3_565 1_445
O8 Ca4 Cl1A Ca1 -54.47(7) 2_645 1_445
P2 Ca4 Cl1A Ca1 128.68(5) 1_545 1_445
Cl1B Ca4 Cl1A Ca1 41.82(6) 1_545 1_445
P3 Ca4 Cl1A Ca1 -143.07(5) 1_545 1_445
O2 Ca5 Cl1B Cl1B -43.7(7) 2_645 3_575
O10 Ca5 Cl1B Cl1B 156.8(6) 1_455 3_575
O1 Ca5 Cl1B Cl1B 21.5(6) 1_455 3_575
O11 Ca5 Cl1B Cl1B -65.3(6) 2_655 3_575
O6 Ca5 Cl1B Cl1B -117.9(6) 2_645 3_575
Cl1A Ca5 Cl1B Cl1B -177.9(7) . 3_575
O7 Ca5 Cl1B Cl1B 86.6(6) 1_455 3_575
P3 Ca5 Cl1B Cl1B -91.1(6) 2_645 3_575
Cl1A Ca5 Cl1B Cl1B -178.4(6) 3_565 3_575
P1 Ca5 Cl1B Cl1B -4.6(7) 2_645 3_575
O2 Ca5 Cl1B Ca4 -174.78(11) 2_645 3_565
O10 Ca5 Cl1B Ca4 25.72(14) 1_455 3_565
O1 Ca5 Cl1B Ca4 -109.54(10) 1_455 3_565
O11 Ca5 Cl1B Ca4 163.61(11) 2_655 3_565
O6 Ca5 Cl1B Ca4 111.06(9) 2_645 3_565
Cl1A Ca5 Cl1B Ca4 51.00(9) . 3_565
O7 Ca5 Cl1B Ca4 -44.45(9) 1_455 3_565
P3 Ca5 Cl1B Ca4 137.88(7) 2_645 3_565
Cl1A Ca5 Cl1B Ca4 50.53(9) 3_565 3_565
Cl1B Ca5 Cl1B Ca4 -131.1(7) 3_575 3_565
P1 Ca5 Cl1B Ca4 -135.68(10) 2_645 3_565
O2 Ca5 Cl1B Ca1 83.68(15) 2_645 3_675
O10 Ca5 Cl1B Ca1 -75.81(14) 1_455 3_675
O1 Ca5 Cl1B Ca1 148.92(11) 1_455 3_675
O11 Ca5 Cl1B Ca1 62.08(10) 2_655 3_675
O6 Ca5 Cl1B Ca1 9.53(10) 2_645 3_675
Cl1A Ca5 Cl1B Ca1 -50.53(9) . 3_675
O7 Ca5 Cl1B Ca1 -145.98(9) 1_455 3_675
P3 Ca5 Cl1B Ca1 36.35(8) 2_645 3_675
Cl1A Ca5 Cl1B Ca1 -51.01(10) 3_565 3_675
Cl1B Ca5 Cl1B Ca1 127.4(7) 3_575 3_675
P1 Ca5 Cl1B Ca1 122.79(10) 2_645 3_675
O2 Ca5 Cl1B Ca1 -87.26(15) 2_645 1_455
O10 Ca5 Cl1B Ca1 113.24(10) 1_455 1_455
O1 Ca5 Cl1B Ca1 -22.02(8) 1_455 1_455
O11 Ca5 Cl1B Ca1 -108.87(9) 2_655 1_455
O6 Ca5 Cl1B Ca1 -161.42(8) 2_645 1_455
Cl1A Ca5 Cl1B Ca1 138.52(15) . 1_455
O7 Ca5 Cl1B Ca1 43.07(8) 1_455 1_455
P3 Ca5 Cl1B Ca1 -134.60(6) 2_645 1_455
Cl1A Ca5 Cl1B Ca1 138.04(7) 3_565 1_455
Cl1B Ca5 Cl1B Ca1 -43.5(6) 3_575 1_455
P1 Ca5 Cl1B Ca1 -48.16(17) 2_645 1_455
O2 Ca5 Cl1B Ca4 -3.34(16) 2_645 1_565
O10 Ca5 Cl1B Ca4 -162.84(9) 1_455 1_565
O1 Ca5 Cl1B Ca4 61.90(8) 1_455 1_565
O11 Ca5 Cl1B Ca4 -24.95(8) 2_655 1_565
O6 Ca5 Cl1B Ca4 -77.50(8) 2_645 1_565
Cl1A Ca5 Cl1B Ca4 -137.56(14) . 1_565
O7 Ca5 Cl1B Ca4 126.99(7) 1_455 1_565
P3 Ca5 Cl1B Ca4 -50.68(5) 2_645 1_565
Cl1A Ca5 Cl1B Ca4 -138.03(7) 3_565 1_565
Cl1B Ca5 Cl1B Ca4 40.4(6) 3_575 1_565
P1 Ca5 Cl1B Ca4 35.76(17) 2_645 1_565
O2 Ca5 Cl1B Ca5 -43.7(7) 2_645 3_575
O10 Ca5 Cl1B Ca5 156.8(6) 1_455 3_575
O1 Ca5 Cl1B Ca5 21.5(6) 1_455 3_575
O11 Ca5 Cl1B Ca5 -65.3(6) 2_655 3_575
O6 Ca5 Cl1B Ca5 -117.9(6) 2_645 3_575
Cl1A Ca5 Cl1B Ca5 -177.9(7) . 3_575
O7 Ca5 Cl1B Ca5 86.6(6) 1_455 3_575
P3 Ca5 Cl1B Ca5 -91.1(6) 2_645 3_575
Cl1A Ca5 Cl1B Ca5 -178.4(6) 3_565 3_575
Cl1B Ca5 Cl1B Ca5 0 3_575 3_575
P1 Ca5 Cl1B Ca5 -4.6(7) 2_645 3_575
